Chemical looping reforming: process fundamentals and oxygen carriers

Chemical looping reforming (CLR) provides a viable process intensification approach for clean and efficient syngas production from carbonaceous fuel with inherent gas–gas separation. The rational design of metal oxide-based oxygen carriers and the scale-up of associated CLR reactor systems play important roles in CLR process development. This review first introduces the concept and advantages of CLR as well as its historical development. The process fundamentals, including basic schemes, reaction stoichiometry, thermodynamics, kinetics and reactor system design, are reviewed. The integral approach for CLR process development is illustrated, showing that the design and compatibility of oxygen carriers and reactor systems are critical for CLR performance. The reaction principle during the reduction of oxygen carriers is discussed, followed by strategies for improving the redox reactivity and stability. We further review and discuss the latest exciting advances on this subject with the purpose of illustrating factors that govern fundamental mechanisms in the redox reaction chemistry of oxygen carriers and their design principles for sustained chemical looping reactor applications. It is expected that these new advances will inspire more effective oxygen carriers and efficient reactor systems for the development and deployment of various CLR processes.

grew by 4.8% as demand for coal, oil and gas rebounded with the economy, reaching 31.5 billion metric tons [1]. Cutting greenhouse gas emissions to limit the increase in average global temperatures to 1.5 ℃ by 2050 is key to averting the worst effects of climate change [6]. A growing number of countries have committed to carbon neutrality strategies to meet the 2050 target. To realize the goal, International Renewable Energy Agency (IRENA) predicted that the annual energy intensity improvement rate needs to rise to 2.9%, nearly 2.5 times the historical trend, and the global energy intensity must reduce by 60% before 2050 [7]. To achieve clean, efficient and cost-effective utilization of carbonaceous fuels, transformative conversion technologies with intensified process schemes, low environmental impacts and high energetic efficiencies are necessary. As shown in Fig. 1, the concept of chemical looping promises to solve these problems in conventional carbonaceous fuel conversion, representing an energy conversion technology that is potentially an affordable, clean and efficient alternative for power generation and syngas [8][9][10][11].
In a broad sense, chemical looping is an approach for process intensification in which a given reaction and/or separation can be decomposed into multiple subreactions via reacting and regenerating chemical intermediates in isolated steps or spaces [12]. The typical design of chemical looping schemes is to integrate reaction and separation with circulating metal oxide-based oxygen carriers in one unit operation and thus intensify the overall process with increased efficiency, lowered emission and reduced cost. In the 1.5 °C Scenario, some emissions persist in 2050 from residual uses of fossil fuels and some industrial processes [7]. Therefore, the remaining CO 2 will have to be captured and sequestered. The concept of chemical looping can be applied for the conversion of carbonaceous fuels to produce electricity, syngas and H 2 with inherent CO 2 control. This concept has been quickly adopted as high-temperature solids looping cycles in the past couple of decades for the in situ removal of CO 2 during the carbonaceous fuel combustion process [3,10,13,14].
In conventional pulverized coal-fired power plants, coal and air are mixed together in the boiler and combusted to release heat while producing a flue gas containing ~ 15% CO 2 in volume. For CO 2 capture from flue gas, a well-established monoethanolamine scrubbing technology could be used, however, it will increase the cost of electricity (COE) by more than 50% [15]. Chemical looping combustion (CLC) is a promising second-generation oxy-fuel combustion technique and has been highlighted as the R&D focus in the European Strategic Energy Plan (SET-Plan) [14,[16][17][18]]. The CLC system mainly consists of a reducer/fuel reactor and a combustor/air reactor, between which oxygen carriers are circulated to convey both heat and oxygen. In the reducer, oxygen carriers provide lattice oxygen to fully oxidize their fuel to CO 2 and H 2 O. A high purity CO 2 stream can be obtained by condensing the water with minimal energy penalty. The reduced oxygen carriers are regenerated with air in the combustor, where sensible heat is released for electricity generation. The CLC approach achieves in situ CO 2 capture during the combustion process, circumventing energy-and cost-intensive air separation and CO 2 separation units. In addition, thermal NO x formation is significantly reduced during its flameless combustion process [19,20]. Techno-economic analysis shows that the CLC process can capture > 90% CO 2 with < 30% increase in the COE while reducing environmentally hazardous pollutants such as NO x [21].
In addition to the CLC application for full oxidation of carbonaceous fuel with in situ CO 2 capture, the CLR process can also be used for partial oxidation to improve the production of CO and/or H 2 . The CLR process has more potential for the chemical and fuel industries due to the wide utilization of CO and H 2 . This review focuses on the research and development of CLR processes and associated oxygen carriers for CO and/or H 2 production from non-solid carbonaceous fuels such as natural gas and alcohol. Chemical looping gasification of solid fuels and thermochemical splitting of CO 2 and/or H 2 O without involving carbonaceous fuels are not discussed in this review [22][23][24][25][26][27]. The concept and advantages of CLR are first introduced and followed by the historical development of related technologies. The various aspects of the CLR

Chemical looping reforming
Conventional reforming process usually consists of a high-temperature catalytic reformer for syngas production, intermediate-temperature water gas shift (WGS) unit for H 2 enrichment, and low-temperature chemical/physical separation for CO 2 removal [5,28]. Taking methane reforming as an example, steam reforming of methane (Eq. 1) is the most common approach, which requires an excess amount of steam to enhance carbonaceous fuel conversion and suppress coke deposition. Consequently, the resulted syngas is rich in H 2 (H 2 :CO molar ratio > 3), which is suitable for H 2 production but not good for fuel and chemical synthesis. Dry reforming with CO 2 (Eq. 2) has been proposed to adjust the H 2 :CO ratio for various downstream applications, but requires excess CO 2 injection to avoid carbon deposition, resulting lower syngas purity. Nevertheless, both reforming reactions are strongly endothermic and carried out in catalytic tubular reactors with external heating (Eq. 3). Such design requires high costs for reactor material of construction and fabrication as well as external fuel combustion to provide the heat necessary to drive the endothermic reactions. Carbon dioxide exists in both syngas from the tube side and flue gas from the furnace side, which complicates carbon capture scheme for natural gas reforming applications. Partial oxidation (POX, Eq. 4) and autothermal reforming (ATR, combination of Eqs. 1,3,4) have also been commercialized for syngas production, which is usually followed by WGS reaction for H 2 enrichment and CO 2 separation for H 2 purification. However, the associated air separation unit (ASU) and acid gas removal unit increase both the energy penalty and capital cost compared to SMR processes.
CLR offers a viable process intensification approach for effective syngas production integrated with in situ gas-gas separation. Figure 1 shows the concept of CLC/CLR for carbonaceous fuel conversion [29][30][31][32][33]. The overall reactions of the CLC and CLR systems are full oxidation (e.g., Eq. 3) and partial oxidation (e.g., Eqs. 1, 2, and 4), respectively. Rational design of CLR reactor system to decouple these reactions and oxygen carriers with high fuel conversion and product selectivity could directly produce high-quality syngas (high CO/H 2 concentrations and desirable ratios) without the need for gas-gas separation units such as air separation and acid gas removal units. For example, Fan et al. [34][35][36][37] developed a three-reactor CLR process, and the overall reaction is the same as the conventional ATR process. Iron-based oxygen carriers are used to convert carbonaceous fuel to CO 2 /H 2 O in a moving bed reducer, and the reduced oxygen carrier then reacts with the steam to directly generate H 2 in a moving bed oxidizer, both of which adopt a gas-solid countercurrent flow pattern in the reactor design. The iron-based oxygen carrier is fully regenerated in a bubbling fluidized bed combustor by reacting with air and then recycled back to the reducer to provide both lattice oxygen and sensible heat. Both CO 2 and H 2 are separated in situ with near zero energy penalty in this three-reactor CLR system, which significantly reduces the separation costs and intensifies the H 2 production processes.
The concept of chemical looping is also advantageous from an exergy point of view [38][39][40][41]. The exergy loss in the carbonaceous fuel conversion process could be reduced by either recuperating the low-grade heat while producing more high-grade heat or designing suitable oxygen carriers in chemical looping processes. As shown in Fig. 2, in the conventional steam methane reforming process, the exergy losses are approximately 12.0% and 8.8% from steam reforming and WGS reactions, respectively. An iron-based CLR scheme is designed and analysed based on the same assumptions [40]. Approximately 5.7% exergy loss occurs in the reducer due to the generation of medium exergy rate iron from low exergy rate iron oxides, and near zero exergy loss is achievable in the oxidizer, as it only requires a small amount of low-grade heat. As a result, the exergy loss for H 2 production using the CLR scheme is significantly reduced compared (1) CH 4  to the conventional process. In summary, through careful design of CLR schemes, significant improvements could be achieved in syngas production and separation with high exergy efficiency and low production cost. These advantages have attracted and inspired tremendous efforts for understanding reaction mechanisms and process fundamentals as well as developing oxygen carriers and reactor systems for various CLR processes.

Historical development of chemical looping reforming
Some representative historical and recent developments of CLR technologies are listed in Table 1. The Howard Lane process was the first industrial application of CLR for H 2 production, which can be traced back to the 1910s [42]. A fixed bed reactor was filled with iron ore and externally heated to reaction temperatures. A mechanical valve system was used for periodic switching between reducing gas (producer gas) and oxidizing gas for conducting redox cycles, a similar pattern used in most current laboratory research. In the Lane process, iron oxide was first reduced with coal-derived producer gas and then regenerated with steam while producing H 2 through the steam-iron reaction. The Lane process achieved an annual H 2 production capacity of 24 million m 3 by 1913 but shortly could not compete with the fast development of natural gas and oil reforming technologies. The low recyclability of iron ores and the poor fuel conversion in the fixed bed reactor system were two critical factors affecting the economics of the Lane process, which reflects that the oxygen carrier and reactor system are the two key components in the development of the CLR process. The steam-iron process was further developed with the use of fluidized bed reactors design to enhance the mass and heat transfer between carbonaceous fuel and oxygen carriers [43]. In the early 1950s, Lewis and Gilliland studied the feasibility of copper or iron oxides as oxygen carriers in a circulating fluidized bed (CFB) system for converting solid fuels to high purity CO 2 [44][45][46][47][48]. Steam and/or CO 2 were used to fluidize the bed materials and promote the reaction between metal oxides and solid fuels in one reactor. The reduced metal oxide was then regenerated by air in a separate reactor. Various reactor designs have been proposed, including multistage fluidized bed, stoker-type or moving bed with gas-solid countercurrent flow pattern, to improve fuel conversion. However, the redox pairs were set to be Fe 2 O 3 /Fe 3 O 4 1 3 scheme in previous studies. Such a scheme decouples the overall reaction of POX or ATR in two reactors. In the reducer, carbonaceous fuel reacts with oxygen carriers forming syngas, and H 2 O and/or CO 2 can be introduced to assist the fluidization and reaction as well as adjust the H 2 :CO ratio. The reduced oxygen carriers are then regenerated in the combustor with air while releasing heat for autothermal operation.
Different types of metal oxides have been investigated under this scheme for CH 4 conversion. Zafar et al. [83] studied the use of SiO 2 -supported Ni, Cu, Mn, and Fe oxides as both reforming catalysts and oxidizing agents. They found that NiO/SiO 2 was the best candidate with high reduction reactivity and high H 2 selectivity. However, the reaction rate decreased as a function of cycle due to the formation of irreversible metal silicates, which do not react at a sufficient rate. Different supports and additive materials have been explored to increase the performance of Ni-based oxygen carriers [84]. Ryden et al. [85] synthesized NiO with MgAl 2 O 4 support and conducted tests in a laboratory reactor consisting of two interconnected fluidized beds. The results showed that NiO/MgAl 2 O 4 had good stability and high reactivity for complete CH 4 conversion and high syngas selectivity, and coke deposition could be reduced or eliminated by 25 vol% steam to methane. He et al. [86] added Fe, Cu and Mn oxides to CeO 2 -based oxygen carriers and showed that the CLR reactivity could be improved with these transition-metal oxides (especially iron oxides) at > 800 °C. However, the fundamental causes of these promotion effects are still unclear.
In addition to CH 4 , the autothermal CLR scheme has been applied for the conversion of other gas or liquid fuels, such as bio oil [87] and ethanol [82]. Dupont et al. [82] studied the CLR of waste cooking oil for H 2 production in a fixed bed reactor with NiO/Al 2 O 3 oxygen carriers. With a high steam-to-carbon molar ratio (S:C) of 4 and a WHSV of 2.64 h −1 , both high fuel and steam conversions could be achieved under a few redox cycles between 600 and 700 °C. Wang et al. [81] investigated the thermodynamic and experimental aspects on CLR of ethanol using a Cu-based oxygen carrier and showed that a H 2 yield of 2.25 mol per mole of ethanol was achieved at 700 °C and a CuO to ethanol molar ratio of 1. Dou et al. [88][89][90][91][92] conducted a series of studies on the CLR of ethanol and glycerol in fixed-bed and moving bed reactors using various Ni-based oxygen carriers between 500 and 650 °C. The results show that the confinement effect by nanostructures could maintain the particle size of Ni-based oxygen carriers and promote their reducibility and reactivity in the CLR process. Recently, Sun et al. [93] prepared Cu 2 O-Ca 2 Fe 2 O 5 oxygen carriers for chemical looping oxidative steam reforming of methanol and realized a high methanol conversion with 40% Cu 2 O sample at 240 °C, due to the suitable catalytic activity and lattice oxygen migration performance. Compared with CH 4 conversion, the autothermal CLR conversion of these biomass-derived liquid fuels can be conducted at lower  temperatures, which reduces the difficulties in maintaining the physical and chemical properties of oxygen carriers and engineering the associated reactor system. Figure 3b and c show the endothermic CLR schemes without oxygen/air feeding. Both schemes require specific considerations of reactor design with external heating. Flue gas containing CO 2 could be generated during the external heating provided with carbonaceous fuel combustion, which defeats the purpose of using the chemical looping concept. Such a dilemma could be avoided by using renewable sources such as biomass and solar energy instead. Furthermore, oxygen carriers that cannot be regenerated by H 2 O and CO 2 are excluded from the endothermic schemes. Specifically, Ni-and Cu-based oxygen carriers that have been widely applied in the first autothermal CLR scheme cannot be used, however, metallic Ni and Cu can still be incorporated, serving as reforming catalysts in endothermic CLR schemes.
The CLR scheme shown in Fig. 3b can be considered as a spinoff of the thermochemical splitting of water and/or carbon dioxide processes, which started around the 1980s [25,26,94]. The original thermochemical redox process consists of high-temperature (> 1300 °C) decomposition of metal oxides releasing O 2 and low-temperature (< 700 °C) reoxidation with CO 2 /H 2 O forming CO/H 2 . The temperature difference between the two steps is too high to carry out the redox cycles in a practical reactor system with sustained oxygen carriers. With the introduction of carbonaceous fuel in the reducer, as shown in Fig. 3b, the reduction temperature could be lowered below 900 °C, and useful syngas could be obtained at the same time. Li et al. [32,95,96] developed a series of perovskite structured oxygen carriers for hybrid water splitting and syngas generation. They rationally optimized the thermodynamic properties of perovskite oxides, including oxygen partial pressure and oxygen vacancy formation energy (E vac ), with the assistance of Ellingham diagrams and density functional theory (DFT) calculations. Experimental studies validated that these perovskite-based oxygen carriers could reach up to 90% selectivity for syngas and H 2 in the reducer and oxidizer, respectively. Li and Zhu found that Fe-Ce mixed oxides had excellent redox performance in methane reforming and water splitting and provided fundamental insights into the redox reaction mechanism and morphology migration of oxygen carriers [97][98][99]. They recently proposed a chemical looping scheme for co-splitting of H 2 O and CO 2 with CeO 2 -LaFeO 3 oxygen carriers, which is efficient and flexible in syngas composition adjustment for various chemical and fuel synthesis [100]. Figure 3c reproduces Galvita and Marin's super-dry reforming process for producing high purity CO from greenhouse gases CH 4 and CO 2 [101]. In addition to using iron oxide as an oxygen carrier, this scheme also adopted nickel as a reforming catalyst and calcium oxide as a CO 2 sorbent. In the reducer, methane dry reforming is carried out over the Ni catalyst, while the resulting syngas is oxidized by Fe 3 O 4 to CO 2 and H 2 O. Under the reducer temperature, CO 2 is in situ captured by CaO, further enhancing the previous two reactions and finally leaving H 2 O as the only effluent gas from the reducer. At the same time, the looping particles change from a mixture of Ni, CaO and Fe 3 O 4 to that of Ni, CaCO 3 and Fe in the reducer. In the oxidizer, external heating is provided to decompose CaCO 3 into CaO and CO 2 , and the latter subsequently reoxidizes Fe back to Fe 3 O 4 . The super-dry reforming scheme can achieve a CO yield of 45% higher than that of the traditional approach, which offers an alternative pathway for efficient CO 2 and CH 4 utilization. Figure 3d and e show three-reactor CLR schemes for H 2 production, where the overall reactions are the same as the autothermal reforming process. Both schemes share similar reactor configurations and produce three hot gas streams containing concentrated CO 2 , high purity H 2 and high-temperature flue gas separately. Such scheme integrates CLC to provide heat for CLR or sorption-enhanced reforming (SER), thus avoiding the external heating needed in the endothermic reforming schemes in Fig. 3b and c. The redox pairs of Fe 2 O 3 -Fe 3 O 4 and NiO-Ni are used for CLC to generate heat, while the pairs of Fe 3 O 4 -FeO/Fe and CaO-CaCO 3 are adopted for CLR and SER, respectively, for H 2 production. More steam usage could cause the overall reaction endothermic compromising the autothermal operation, while more oxygen usage could generate excess heat, sacrificing the H 2 yield. Based on the heat of combustions and reforming reactions and thermodynamic equilibrium, the minimal oxygen and steam usage could be estimated for the design and optimization of three-reactor CLR reactor systems.
The iron-based three-reactor CLR scheme shown in Fig. 3d specifically represents the SCL process developed by Fan, which can coproduce H 2 and electricity with high efficiency. In the reducer, iron-based oxygen carriers are used to fully convert syngas or natural gas into H 2 O and CO 2 , and Fe 2 O 3 is reduced to a mixture of Fe and FeO at approximately 900 °C. The oxidizer operates below 800 °C to conduct steam-iron reaction to produce high purity H 2 and reoxidize the reduced iron to Fe 3 O 4 . The combustor then completely regenerates Fe 2 O 3 oxygen carriers and provides heat for autothermal operation. From the iron-based three-reactor CLR scheme, three hot gas streams are produced: a concentrated H 2 O/ CO 2 stream from the reducer, a H 2 O/H 2 stream from the oxidizer and the flue gas stream from the combustor. The flue gas could be sent to an expander to recover the high-grade heat, and the exhausted gas, together with the other two streams, is routed to the heat recovery and steam generation section. After condensing out the steam, high purity CO 2 1 3 and H 2 streams can be obtained separately. The SCL process is more efficient than the conventional process due to its efficient energy management and integrated CO 2 separation scheme. Figure 3e shows the scheme of sorption-enhanced chemical looping reforming (SECLR), which is the combination of SER and CLC. SER for H 2 production can be accomplished by the addition of CO 2 sorbent (e.g., CaO) for in situ CO 2 removal and thus driving the steam reforming and WGS reaction equilibrium towards H 2 -rich products, while CLC can be achieved by the addition of oxygen carriers (e.g., NiO) to provide lattice oxygen and catalytic sites (reduced Ni) for fuel reforming. Calcium carbonate can be separately calcined to yield a pure CO 2 stream for its subsequent sequestration, and the calcium-based sorbent can be regenerated and recycled back. The nickel-based oxygen carrier can be regenerated with air to provide heat for the reforming reaction as well as the calcination reaction. By applying this scheme, higher H 2 yield and purity can be directly obtained with in situ CO 2 capture using reusable sorbents and metal oxides without additional gas-gas separation units.
Dupont et al. [102] The results showed that > 95% purity of H 2 was produced at 600 °C and 1 atm. Zeng et al. [103] conducted SE-CLR of ethanol with Ni-based catalyst and CaO sorbent and studied the NiO loading as well as reaction conditions of the reforming reactor. Increasing NiO loadings could lead to higher catalytic activity as it provided more active surface sites to accelerate intermediates to H 2 and CO. The highest ethanol conversion and H 2 selectivity were obtained at 650 ℃ with 20% loading of NiO, achieving a conversion of 98% and H 2 selectivity of 93%. Dou et al. [92] revealed that high purity H 2 production from glycerol could be achieved via SECLR using a continuous dual moving-bed reactor over NiO/ NiAl 2 O 4 oxygen carriers and lime-based sorbent. Hafizi et al. [104] investigated the performance of Fe-Ce-based oxygen carriers and CaO-based sorbents on the SECLR of CH 4 using a fixed-bed reactor. The results showed that H 2 purity of 89% could be obtained at 600 °C, S:C ratio of 1.5 and sorbent to oxygen carrier mass ratio of 3. Recently, they applied Co 3 O 4 / SiO 2 oxygen carrier and a cerium-promoted calcium-based sorbent in the SECLR process, and showed that up to 95% H 2 purity could be achieved at 550 °C, which is comparable to 84% in the CLR process [105]. Also, formic acid was realized as a prospective hydrogen carrier, and a sodium looping-based formic acid reforming was proposed and simulated for high-purity H 2 production. Conditions, i.e., temperature, pressure, and ratio of H 2 O/HCOOH as well as Na 2 CO 3 /HCOOH, for three reactors were optimized to promote H 2 production and CO 2 absorption. Results showed a high H 2 production rate with a high purity of 97.9% and an ultra-low CO concentration of 11.97 ppm [106]. The continuous operation of all three reactors, however, has not yet been demonstrated in the SECLR process. With three interconnected fluidized bed reactors simultaneously exchanging a mixture of two looping particles, i.e., the CO 2 sorbent and the oxygen carrier, the operation and control requires a systematic approach. Issues that need to be further addressed include the simultaneous handling of mixed sorbent and oxygen carrier, sorbent and oxygen carrier reactivity and recyclability, heat transfer and solid/gas leakage among the reactors.

Product selectivity: stoichiometry, thermodynamics and kinetics
The product selectivity, i.e., the concentration and ratio of H 2 and CO in the syngas, in a CLR process could be affected by many factors, including reaction stoichiometry, thermodynamic equilibrium, surface reaction path and reactor system configuration. The reactor system configuration has been briefly discussed in the previous section. For example, the three-reactor CLR system could be designed to directly produce both H 2 and CO 2 in high purity from separate reactors, as shown in Fig. 3d and e. Amini et al. [80] have recently reviewed the effect of pressure in chemical looping system, concluding that high pressure is beneficial for the reaction kinetics and hydrogen production process. More review and discussion on the effect of reactor system configuration are addressed in Sect. 2.3.
The overall reaction stoichiometry determines the syngas selectivity and H 2 :CO ratio based on the fuel and oxidant input. Based on Eqs. 1, 2 and 4, the theoretical H 2 :CO ratios in the syngas from steam reforming, dry reforming and partial oxidation of methane are 3:1, 1:1 and 2:1, respectively. The contents of C, H, and O elements in other carbonaceous fuels, such as biomass-derived oil and alcohols, could vary to certain extents. Accordingly, the syngas composition could be adjusted for different downstream applications by varying the stoichiometric ratios of different feedstocks introduced to the CLR system. As discussed in the previous section, the stoichiometric ratio also determines the heat of the overall reaction based on the first law of thermodynamics.
As a chemical looping process consists of cyclic gas-solid reactions, successful operation relies on the performance of the oxygen carriers. In a typical chemical looping scheme, the overall reaction can be regarded as combustion and partial oxidation/reforming of the fuels, which requires distinct oxygen carrier properties so that the product selectivity can be properly controlled. For example, with a substoichiometric ratio of available lattice oxygen to fuel, partial oxidation of hydrocarbons for syngas production could be performed by metal oxides such as NiO and CuO. However, the resulting syngas concentration is highly dependent on the oxygen-to-fuel ratio in this case. The second law of thermodynamics suggests that the reaction equilibrium could vary significantly with different oxygen carriers and operation conditions. The performance of oxygen carriers, typically metal oxides, can be estimated based on their equilibrium oxygen potential at high temperatures. The oxygen potential of various metal oxides could be studied and categorized with ease via the Ellingham diagram or the oxygen partial pressure diagram, as shown in Fig. 4 [107]. The corresponding oxygen partial pressure for combustion and reforming/gasification of representative fuels such as CH 4 , C, CO and H 2 are also included. The active metal oxides could be sorted into the following groups.
The combustion or CLC group, including the oxides of manganese, iron, copper, etc., is located at the top pink zone of Fig. 4, where metal oxides have strong oxidizing capability. These metal oxides could be used as active components in oxygen carriers for complete fuel oxidation to CO 2 and/or H 2 O in CLC processes, as their oxygen partial pressures are above the lines of CO and H 2 combustion. Molecular oxygen could be directly generated by exposing metal oxides such as Mn 2 O 3 , Co 3 O 4 and CuO at high temperatures where their decomposition oxygen partial pressure could exceed 0.01 bar, which could facilitate the conversion of solid fuels in the so-called chemical looping with oxygen uncoupling (CLOU) process [108]. In contrast, the lines of CaSO 4 , NiO and CoO are near the bottom of this zone, indicating that there is a small portion of uncovered fuel present in the reduction step. In general, the oxygen carriers in this group are mostly studied for CO 2 capture-oriented CLC processes.
The CLR group is in the blue zone located below the CLC group and above the line of CO formation. Thus, metal oxides in this region are able to gasify carbon to CO but cannot further oxidize CO and H 2 due to their moderate oxidizing capability. As a result, metal oxides in this group can be used for syngas production from various carbonaceous fuels. The advantage of using metal oxides in the CLR group is that they can thermodynamically ensure the stable production of high purity syngas while minimizing carbon deposition [33]. The inset of Fig. 4  The third group is located at the bottom zone of Fig. 4, where the metal oxides have limited or no oxidation capability. This group is able to partially or selectively oxidize hydrocarbons. However, coke deposition or incomplete fuel conversion is inevitable. Metal oxides in this group can also be used as support materials such as TiO 2 , SiO 2 and Al 2 O 3 . Under reaction conditions, the support could interact with the abovementioned active metal oxides in many ways. For example, iron oxides can also react with TiO 2 , SiO 2 and Al 2 O 3, forming FeTiO 3 , FeSiO 3 and FeAl 2 O 4 , which could alter their thermodynamic and kinetic properties during chemical looping applications. Specifically, ITCMO oxygen carriers have been selected to improve the syngas selectivity and yield with minimal carbon deposition based on the following thermodynamic analysis [33].
The ratio of reducible oxygen provided by the metal oxides to CH 4 ([O]:CH 4 ) significantly affects the syngas composition and the possibility of carbon formation. As shown in Fig. 5, for both iron oxides and ITCMOs, when this ratio is lower than 1, a substoichiometric amount of oxygen is provided, which results in possible carbon deposition, carbide formation, :CH 4 ratio is higher than 1, most of the carbon is converted to either CO or CO 2 . Figure 5a shows that iron oxide can achieve a low CO 2 selectivity (< 15%) when the [O]:CH 4 ratio is below 1.5. Under such conditions, however, metallic iron is the only reduced solid product and can catalytically decompose CH 4 , causing carbon deposition. Carbon deposition/formation may be avoided by reducing the extent of metal oxide reduction by increasing the [O]:CH 4 ratio. Conversely, increasing this ratio results in an increase in CO 2 and H 2 O levels to more than 30 mol%, lowering the syngas selectivity and yield. Thus, the use of single metal oxide material poses challenges in syngas quality control.
The ITCMO oxygen carriers possess a better equilibrium property toward syngas generation. With proper iron oxide and titanium oxide ratio, the effective reduced compounds can be FeTiO 3 and/or Fe 2 TiO 4 . As shown in Fig. 5b, ITCMO with a Fe to Ti ratio of 2 can partially oxidize CH 4 to syngas with minimal byproducts such as C, CH 4 , CO 2 and H 2 O. Unlike single metal oxide materials such as FeO, the syngas composition produced using ITCMO is very stable and of high concentration (> 90% CO selectivity) when the [O]:CH 4 ratio varies in a wide range between 1.5 and 4. Without any steam injection, the CH 4 reaction with ITCMO can produce syngas at a H 2 :CO ratio slightly below 2. The H 2 :CO ratio can be improved to 2 by introducing steam at 10% of the CH 4 molar flow. In the conventional autothermal reforming process, a steam-tomethane ratio of more than 20% is required to obtain a similar syngas composition. Thus, the ITCMO is promising for high-efficiency, high-quality syngas production.
In summary, the diagram of equilibrium oxygen partial pressure can guide the selection of active components and estimate the syngas selectivity preliminarily in CLR system. Nevertheless, the syngas selectivity could be also affected by the selection of supporter, ionic diffusion and catalytic kinetics, which will be further reviewed and discussed in Sect. 3.

Reactor system design
The reactor system design plays a critical role in determining the chemical looping process performance. It has been widely recognized that the combustor or air reactor should be operated in a fluidized bed mode for better heat and mass transfer, and the associated reactions are intrinsically fast and are thermodynamically favored. However, unlike the oxidation reaction in the combustor, the reactions with carbonaceous fuel in the reducer are complicated and could be limited by thermodynamic equilibrium and be relatively slow. It is therefore necessary to study the gas-solid contacting pattern and to optimize the reducer design, targeting high reliability and low capital-intensity while maximizing solid and gas conversions.
Based on the feeding mode, chemical looping reactor systems can be categorized into batch reactor system with gasswitching mechanical valves and circulating bed system with continuous gas and solid flow. A variety of reactor designs with different Geldart particle grouping and solid flow behaviors have been developed, including fixed bed, moving bed, and fluidized bed [12,16,109]. Among these reactors, the fixed bed reactor is simple in its design, and poses the least requirements on the mechanical strength of oxygen carrier particles. Thus, fixed bed has been widely used in lab-scale tests and was first commercialized in the Lane process for H 2 production [42]. However, fixed bed reactors can only handle gaseous fuel and require frequent gas switching at high temperatures, which is not suitable for large-scale operation. In addition, the poor heat transfer between gas and solids in the fixed bed reactor could cause hot spots that further lead to sintering and deactivation of oxygen carriers. To solve these problems, researchers have developed alternative reactor systems for continuous chemical looping operation. Figure 6 shows three major types of gas-solid contacting patterns for chemical looping reactors, which include mixed flow, countercurrent flow, and cocurrent flow. The mixed flow pattern mainly occurs Reproduced from ref. [33] with permission from the Royal Society of Chemistry, copyright 2014 in the single-stage fluidized bed reactor, while the countercurrent and cocurrent flow patterns could be achieved in a moving bed or a series of interconnected fluidized bed system.
To date, various fluidized bed configurations, such as bubbling-, turbulent-and spout-fluidized bed operations, have been applied to provide good mixing characteristics and uniform heat transfer in CLC applications. However, back mixing and channelling in a fluidized bed usually results in poor fuel conversion and low product purity, and the separation among oxygen carriers, solid fuel and ash remain a major challenge. These aspects are closely related to the reaction kinetics between carbonaceous fuels and oxygen carriers as well as the design and operation of chemical looping reactors. Song and Shen reviewed the solid fueled CLC reactor system, and suggested proper design of the feeding position and bed internals to address operational problems [16]. Zhao et al. [109] recently updated their progress in chemical looping process development, and emphasized the importance of numerical simulation in the design, optimization, and scale-up of fluidized bed reactors. In the following, the fundamental and design of two iron-based CLR moving bed reactor system, i.e., the STS process and the SCL process, are discussed.
The STS process produces syngas from shale gas via the redox cycle of ITCMO oxygen carriers discussed in the previous section. To make full use of the thermodynamic properties of ITCMO oxygen carriers, a cocurrent moving bed reducer design is adopted [33]. The cocurrent gas-solid contact configuration controls the proper redox time and the extent of the oxygen carrier conversion while preventing carbon deposition. At the inlet of the reactor, the concentrated fuel source reacts with Fe 2 TiO 5 /Fe 3 O 4 , which is highly oxidative and unlikely to catalyze carbon deposition. At the outlet of the reactor, although reduced oxygen carriers contain metallic Fe, the atmosphere of diluted fuel and the lattice oxygen in Fe 2 TiO 4 /FeTiO 3 could help prevent carbon deposition. The reduced ITCMO consisting of Fe and Fe 2 TiO 4 /FeTiO 3 yields a corresponding thermodynamically high syngas purity with a H 2 :CO ratio of ~ 2:1. The cocurrent moving bed reducer is advantageous over a fluidized bed reducer in that the moving bed reducer does not suffer a reduced shale gas conversion and/or undesirable syngas composition due to gas channelling and back mixing of particles with different oxidation states, which are unavoidable in a fluidized bed reactor. A set of experiments was conducted to characterize the ITCMO performance and validate the cocurrent moving bed concept [33].
The SCL scheme is shown in Fig. 3d, in which high syngas conversion and high steam-to-hydrogen conversion are two of the most important criteria for evaluation. In a fluidized-bed reactor such as a dense-phase fluidized bed, significant gas and solid mixing occurs. Thus, in a fluidized-bed reducer, the fresh syngas feedstock is diluted by the gaseous product, which is rich in H 2 O and CO 2 . Table 2 lists the equilibrium compositions between FeO x and CO/CO 2 /H 2 /H 2 O at 850 °C, indicating that the dilution of the syngas by CO 2 and H 2 O decreases the reducing capability of the syngas. For example, in order to achieve 100% conversion of syngas, iron oxides cannot be reduced to an oxidation state lower than Fe 3 O 4 . This indicates that the

3
Fe 2 O 3 conversion cannot be higher than 11% with 100% syngas conversation in a fluidized bed reducer. Therefore, the gas and solid conversions in the fluidized-bed reducer are constrained. Contrary to the fluidized bed reactor, a moving bed reactor has minimal axial mixing between the gas and solid phases. The SCL process uses a moving bed reactor with a countercurrent gas-solid contacting pattern for the reducer design. Based on the thermodynamic data shown in Table 2, at the bottom of the moving bed reducer, a fresh syngas feed with high H 2 and CO concentrations could react with iron at lower oxidation states. Meanwhile, the partially converted syngas with low H 2 and CO concentrations flows upward to meet iron at higher oxidation states. A multistage equilibrium model has been developed for the countercurrent moving bed reactor, which predicts that 100% syngas could be converted and Fe 2 O 3 could be reduced by ~ 50% to a mixture of Fe and FeO [74]. Thermodynamic analysis has attempted to provide insight into the operational conditions of the SCL system using a moving bed reducer. The theoretical results confirm that the gas-solid countercurrent moving bed reducer with iron oxide oxygen carriers can achieve high fuel conversions to CO 2 and H 2 O with a minimal solid circulation rate, is resistant to carbide and sulfide contamination, and has the capability of producing high purity H 2 .
Furthermore, a one-dimensional dynamic model was developed to simulate the moving bed reducer in the SCL process [70,110]. As shown in Fig. 7a, the bench-scale experimental data validated both the multistage equilibrium model and the 1-D dynamic model [70]. Both experimental and modeling results show that the gas and solid conversion profiles have opposite trends because of the countercurrent contact pattern. Under the current operating conditions and reducer design, an individual particle quickly completes the reduction from Fe 2 O 3 to Fe 3 O 4 and then to FeO at the top. The reduction from FeO to Fe is then limited by thermodynamic equilibrium before the gas profile is changed at the bottom, where fresh syngas is introduced. The steady-state simulation results with different reducer heights are shown in Fig. 7b. The results suggest that there is a minimal height to achieve the same reducer performance. In summary, the 1-D movingbed reactor model provides insights into optimizing the countercurrent moving bed reducer design and operation.
The above examples illustrate the integral approach for the iron oxide based circulating moving bed CLR process development. Adanez et al. [2] have reviewed the progress in chemical looping combustion and reforming technologies, including various reactor and process development up to 2010. Most existing CLR processes proposed dual fluidized bed reactor design for high temperature natural gas reforming applications. In recent years, gas-switching concept was also studied to avoid solids attrition and circulation problems in the scale-up process [80]. Such system requires high temperature mechanical valves, which is practical for temperatures below 600 °C and could be applied for the CLR of oxygenated fuels including methanol [111,112], ethanol [113,114], etc. Various reactor configurations and associated experimental results are out of the scope of this review, and related discussion could be found from recent reviews [16,80,109].
In summary, the basic schemes and process fundamentals of the CLR system are discussed. The reaction stoichiometry, thermodynamic equilibrium, and reactor system configuration are all factors that could affect the gas product yield, and selectivity in the CLR. Besides, the gas-solid contacting pattern should be carefully considered and selected for specific CLR applications.

Reaction principle
The reduction and oxidation of oxygen carriers generally involve the generation and recombination of oxygen ions and vacancies, their diffusion in the bulk phase, and their reaction with adsorbed species on the surface. Transition metal oxides such as NiO and CuO have been widely studied as oxygen carriers, and the reduced metals are also effective catalysts for the conventional reforming processes of various fuels. For example, methane and ethanol reforming could be catalysed by metallic Ni at 700-900 °C and 400-600 °C, respectively, while methanol can allow the reforming process to operate at a relatively lower temperature around 100-300 °C with Cu catalyst. Suitable oxygen carriers would employ active metal for its high reactivity and temperature compatibility with corresponding fuels. Figure 8 schematically shows the reaction principle of oxygen carriers under a reducing environment. In the first step, the metal-oxygen bonds in oxygen carriers are activated by absorbing thermal energy at high temperatures, resulting in oxygen ions and vacancies as well as electron-hole pairs. This relates to the thermodynamic property or oxygen potential of the metal oxides, as discussed in the previous section. Metal oxides in the CLC and CLR groups of Fig. 4 are the active oxygen carrier components, and their oxidizing capability could determine the fuel conversion and product selectivity. Foreign metals could be used to modify the thermodynamic properties and facilitate redox reactions at low temperatures. The screening and discovery process could be accelerated with computational chemistry methods and high-performance computing systems. For example, Li et al. [96] rationally designed BaMn x Fe 1-x O 3-δ oxygen carriers and optimized their redox thermodynamic properties, including equilibrium oxygen partial pressure and E vac , with the assistance of DFT calculations and Ellingham diagrams. The experimental results showed that up to 90% selectivity of syngas and H 2 could be achieved in the reducer and oxidizer, respectively, indicating that BaMn x Fe 1-x O 3-δ oxygen carriers are promising for efficient solar-driven CLR process.
In the reducing environment caused by the fuel, the activated oxygen anions diffuse from the bulk phase to the surface under the oxygen chemical potential gradient. At the same time, electrons flow inward to maintain the overall charge neutrality. The ionic diffusion in the bulk phase determines the release and replenishment rate of lattice oxygen. Most oxygen carriers revolve around only a few crystal structure types, such as fluorite and perovskite. In perovskite oxides with more open oxygen sublattices, oxygen vacancies can be created more easily than cation defects. Consequently, perovskite oxides show high lattice oxygen diffusivities, which is suitable for various CLR processes [32,95,[115][116][117][118][119][120][121][122]. Metal oxides with fluorite structure such as CeO 2 have predominantly oxygen anion defects occupying interstitial sites. The removal of lattice oxygen atoms on ceria could lead to the formation of several phases of the type CeO 2−x with a range of possible compositions (0 ≤ x ≤ 0.5). This feature can be used to form solid solutions with oxygen vacancies by substituting aliovalent ions of the host structure with a higher charge than that of the replacing cation, and has been applied in oxygen carrier development for CLR applications [25,123,124]. Thus, specific crystal structure and bulk doping can be used to improve the ionic diffusion rates. Surface reactions take place between the adsorbed fuel species and oxygen species diffused from the bulk phase. Catalytic sites could be formed during the reduction of the oxygen carriers or specifically introduced to the surface to promote the reaction kinetics. Fuel conversion and syngas selectivity in the CLR reducer could be improved by controlling the distribution of oxygen supply from the bulk as well as the types of active oxygen species on the surface. It is noted that coke deposition frequently occurs in the reforming process, and if the oxygen supply from the bulk is inadequate, coke could be accumulated on the surface of oxygen carriers and lead to deactivation. While lattice oxygen atoms participate in the oxidation of carbonaceous feedstock, they do not necessarily result in high product selectivity. The selectivity is based on the bond strength between the metal atom and the lattice oxygen atom on the surface. If the metal-oxygen bond is too weak, lattice oxygen can be easily released so that the reactant adsorbed on the surface may be fully oxidized to yield CO 2 and H 2 O. If the metal-oxygen bond is too strong, lattice oxygen atoms cannot be released, which could result in a low reactivity. Ideal oxygen carriers with readily mobile lattice oxygen and suitable metal-oxygen bond strength have the potential to be both selective and reactive.

Effects of the promoters
The CLR process requires oxygen carriers to exhibit both high fuel conversion and high syngas reactivity, along with low cost and high stability at high temperatures. Extensive efforts have been devoted to catalytically modifying the surface for performance improvement. Fan et al. [125] studied the idea of using metal oxide dopant at a very low concentration relative to the total metal oxide oxygen carriers (e.g., < 1%) without yielding phase change to reduce the energy barrier of carbonaceous feedstock activation and hence facilitate carbonaceous feedstock conversion. They modified the Fe 2 O 3 oxygen carrier using 1% lanthanum dopant and found that it could enhance redox reactivity while maintaining the high oxygen capacity and recyclability of oxygen carriers. The reactivity of La-doped iron oxide oxygen carriers is higher than that of undoped iron oxide oxygen carriers by 220% for CO reduction reactions and 260% for air regeneration reactions. In addition, 1% La dopant led to a 178% increase in reduction reactivity and a 156% increase in reoxidation reactivity for CH 4 reforming reactions compared to undoped iron oxide. The mechanism for La dopant-based reactivity enhancement stems from the capability of La dopant in lowering the barriers of C-O bond and C-H bond activation during metal oxide redox reactions with carbonaceous fuels. Furthermore, they found that the low concentration aliovalent dopant modification can more significantly improve CH 4 conversion on iron oxide oxygen carriers. Fan et al. [126] doped iron-based oxygen carriers with a small amount of cobalt, and the addition of trace amounts of cobalt significantly increased the activity of the oxygen carriers in the 600-800 °C range, which is beneficial for low-temperature applications of iron-based oxygen carriers. The introduction of cobalt can prompt the formation of oxygen vacancies, which affects the energy barrier of CH 4 reforming on the surface of the oxygen carriers.
In addition to modifying the active sites on the surface/interface to improve the reactivity and selectivity, promoters also can be adopted for modifying the bulk phase structure to improve oxygen vacancy formation and ionic conduction. Chen et al. [127] recently demonstrated that tungsten-based oxygen carriers with nickel modification were effective for the CLR of CH 4 . Their results indicated that the oxygen availability, CH 4 conversion, and syngas yield could be significantly increased over Ni 0.5 WO x /Al 2 O 3 compared to WO 3 /Al 2 O 3 . Further investigations showed that there is a strong interaction between surface-grafted nickel species and WO x species, effectively improving CH 4 activation and the surface reforming reaction. At the same time, nickel was incorporated into the bulk structure of WO 3 , which weakened the tungsten-oxygen bond strength and increased the availability of lattice oxygen. As a result, the syngas yield was significantly increased by ~ 2.7-fold in comparison with unmodified WO 3 oxygen carriers. These findings are a pathway to dramatically modify metal oxide properties using relatively simple fabrication processes, and they significantly impact future chemical looping oxygen carrier design.
Even though much effort has been taken into the modification of oxygen carriers by different approaches, there is still a long way to explore the reaction mechanism more explicitly for CLR applications. The reactions with oxygen carriers involve the generation and transfer of different oxygen species from the bulk phase to the surface and variation of these parameters determines the specific reaction pathway on the surface, thus resulting in different products. By modifying the bonding energy between adsorptive intermediates and metal-oxygen bonds, which are significantly dependent on the distribution and diffusion of various oxygen species, the distribution of products can be modulated.

Oxygen carrier deactivation
The deactivation of oxygen carriers remains the major problem for CLR applications [128]. In general, the deactivation of oxygen carriers in the CLR process can be analyzed from microscopic and macroscopic aspects. At the microscale, the deactivation of the oxygen carrier is mainly caused by the sintering of active components, thermal inactivation, oxygen carrier poisoning due to contaminant mineral matter in the fuel, carbon deposition and lattice oxygen depletion, which leads to changes of the surface and bulk phase of the oxygen carrier. At the macroscale, deactivation mainly includes changes of textural properties and the decline in mechanical strength.
The high temperature of the CLR process could lead to severe surface sintering of the oxygen carrier, especially the supported oxygen carrier. As a result, the crystal grains of the oxygen carrier grow, and the dispersion of the active component on the surface decreases, thus reducing the surface area of the active component [4,129]. In addition, sintering could increase the oxygen transmission distance inside the oxygen carrier, causing difficulties in lattice oxygen diffusion. Moreover, the number of active sites of the oxygen carrier is also reduced due to the decrease of lattice imperfection during sintering. Therefore, it is crucial to solve the irreversible sintering of the oxygen carrier. At present, the solution to the sintering problem is mainly realized by optimizing the preparation method and adopting the carrier with high specific surface area and excellent pore structure to obtain the oxygen carrier with smaller grain size while inhibiting grain growth in the reaction process [4,[130][131][132]. At the same time, the addition of structural promoters could also effectively suppress the sintering of the oxygen carrier.
Thermal inactivation is also a major cause of oxygen carrier deactivation. At high temperatures, the components of oxygen carriers undergo solid-phase reactions to produce substances with poor reactivity and low oxygen storage capacity, and oxygen carriers may also undergo phase transition and phase separation. All these factors could cause a decrease of the activity of the oxygen carrier and eventually lead to inactivation. For example, Al 2 O 3 support tends to undergo solid-phase reaction with transition metal oxides at high temperatures [133,134]. Therefore, when Al 2 O 3 is used as the support, it is found that the performance of the oxygen carrier decreases with the increasing number of cycles [135,136]. Most of the literature attributed the decline in activity to the production of aluminate because aluminate has a lower oxygen storage capacity and reactivity. In addition, due to the formation of aluminate, the metal oxide cannot be completely reduced so that the amount of available oxygen is reduced, resulting in the reduction in conversion and syngas yield. To solve this problem, supports with weak interactions between active components such as MgAl 2 O 4 spinel can be selected, or strong oxidants such as oxygen can be used to fully oxidize aluminate back to its original form [137][138][139][140].
When zirconia is used as the support, the phase change during the high-temperature reaction causes cracks in the structure and issues in the mechanical properties [141]. Zirconia can be stabilized by adding additives such as MgO or CeO 2 , thereby solving the problems caused by its phase transition [128,142]. For phase separation, titanium and iron in the ilmenite structure undergo phase separation. As the reaction progresses, iron oxide gradually accumulates on the surface, while titanium dioxide is gradually enriched in the bulk phase, which affects the cycling stability of the oxygen carrier. The introduction of an Al-based skeleton can solve the phase separation problem of ilmenite-based oxygen carriers [143].
Compared to sintering, carbon deposition is a reversible deactivation because carbon deposition can be eliminated to a certain extent in the oxidation stage. In addition, when CO 2 or steam is selected as the oxidant, CO 2 and carbon deposits can be fully utilized to increase the yield of carbon monoxide. The mechanism, pathway, amount, and composition of carbon deposition vary with oxygen carriers and CLR reactions. However, the specific surface area, pore volume and active center of the oxygen carrier could decrease with the increase of carbon deposition and lead to deactivation of the oxygen carrier. The generation of carbon deposition is mainly caused by the acid center and slow oxygen migration rate in the oxygen carrier. Therefore, in addition to reducing the acid center in the oxygen carrier to reduce carbon deposition, the formation of carbon deposition can also be inhibited by accelerating the transfer of lattice oxygen [144,145]. The addition of a certain amount of additives, such as adding Sr to the A site of the perovskite oxygen carrier to obtain more oxygen vacancies [118,146], and adding zirconia with a smaller ion radius to cerium oxide to cause lattice distortion [147,148], can reduce the activation energy of the diffusion of oxygen ions and is beneficial to the migration and diffusion of lattice oxygen. Therefore, the carbon deposits on the surface can be eliminated in time to avoid deactivation of the oxygen carrier. In addition to modifying the oxygen carrier, the production of carbon deposits can also be suppressed by optimizing the reaction conditions. Adding an appropriate amount of steam or CO 2 to the reactants or immediately entering the oxidation stage after the carbon 1 3 deposits are generated can avoid carbon deposits or inhibit the deactivation caused by carbon deposits to a certain extent. A suitable operation pressure is also desired to alleviate the carbon deposition as pressure has a great influence on the deactivation of oxygen carriers. High pressure can lead to fast deactivation by accelerating the carbon deposition on oxygen carriers especially for Ni-and Fe-based ones [149,150].
The deactivation of the oxygen carrier at the macroscale is mainly caused by the change of the texture characteristics and the decrease in mechanical strength. Both active metal oxides and the support could sinter at high temperatures, causing the change in the texture characteristics of the oxygen carrier. With the increase of temperature and the extension of reaction time, the micropores of the support undergo sintering, which in turn causes an increase in the average pore diameter and decreases in the total porosity and the specific surface area. With the change of the texture characteristics, the contact area of the active components with the reactants decreases, which significantly reduces the performance of the oxygen carrier. When oxides such as CeO 2 are used as the support, the sintering of the support not only affects the macroscopic properties but also reduces the oxygen transport capacity of the support, thereby affecting the overall oxygen transport capacity of the oxygen carrier. To maintain the texture characteristics, a series of preparation methods have been developed and optimized [151]. The abrasion and spalling of the oxygen carrier are closely related to its mechanical strength. For oxygen carriers, the improvement of mechanical strength can be achieved by adding additives and supports or optimizing the preparation method [151].
In addition to the deactivation of the oxygen carrier, the low selectivity of the oxygen carrier to the target product is also a factor affecting its development. Taking chemical looping methane reforming as an example, when oxygen or air is used as the oxidant, the surface oxygen of the oxidized oxygen carrier is restored, and thus, the selectivity of the complete oxidation product is increased, which is undesirable. Therefore, in order to solve this problem, the oxygen carrier can be selectively oxidized by reducing the oxidation time [132] or using a weak oxidant such as CO 2 [152] to restore the oxygen related to partial oxidation, thus increasing the selectivity of the target product. Continuous effort will be devoted to improving the long-term redox stability of oxygen carriers.

Primary material selection
Oxygen carriers are at the heart of chemical looping process development, which can circulate between two or more reactors/steps and convert raw materials into target products [9]. Since CLR uses oxygen conveyed by the oxygen carrier, they usually consist of metal oxides able to react with fuels such as CH 4 . On account of the original purpose of CLR is to avoid the inadequacies of conventional steam reforming, partial oxidation, and autothermal reforming technologies, and to obtain a synthesis gas with a suitable H 2 /CO ratio, the oxygen carrier should have a better fuel conversion rate and higher selectivity. In this regard, we can roughly perform a simple screening through the Ellingham diagram. The Ellingham diagram classifies and studies the thermodynamic properties of oxides based on their equilibrium oxygen potentials. The products of metal oxides reacting with the raw materials and their selectivity can be estimated based on their thermodynamic properties from the Ellingham diagram [9]. In addition to the Ellingham diagram, high-throughput thermodynamic screening technology can also be used to screen oxygen carriers [153]. The technology adopts the Gibbs energy descriptor [G δ (T)], which only needs information about the composition, enthalpy of formation and atomic density of the material. The descriptor can be used to predict the Gibbs free energy that reacts with CH 4 , thus obtaining the corresponding conversion. Since the prediction method is only sensitive to parameters such as temperature, and the material category has little influence on it, this method can be widely applied to chemical looping processes and has similar accuracy on various materials under equilibrium or near equilibrium situation. Li et al. [154] recently reported the oxygen chemical potentials for over 2000 perovskite oxides were simulated as a function of their oxygen vacancy concentrations and more than 100 materials were predicted to be applicable. Among the potential candidates, intriguingly, "nonobvious". The phase diagram thermodynamic database can be used to computationally study the water conversion capability of metal oxides for chemical looping hydrogen generation [155]. In addition to screening for suitable oxygen carriers, the DFT method was used to screen for dopants, thus providing a fuller understanding of the selection of dopants [156,157].
Previous studies show that most transition metal oxides agglomerate or sinter rapidly without the addition of additives or supports, resulting in a loss of available metal oxide sites. Considering that the long-term operation of CLR is to realize the industrialization of the process, another requirement is that the oxygen carrier should maintain both physical and chemical stability over multiple cycles under reaction conditions. In addition, the cost, toxicity, thermal stability, and attrition resistance of the oxygen carrier are also factors to be considered for industrialization. Specific to the requirements of laboratory-scale development for oxygen carriers, we need to maintain a high conversion, a high selectivity of H 2 and CO, and a low selectivity of CO 2 and carbon deposition. For chemical or fuel synthesis purposes, the H 2 /CO ratio is better at around 2. In addition, fresh and spent oxygen carriers can be characterized by XRD and TEM to check whether the crystal phase or structure is stable and the variation in the particle size. Among all transition metals, nickel-, iron-, and cerium-based oxygen carriers are commonly used in the field of CLR (Fig. 9). These oxygen carriers have their own advantages and disadvantages. Ni-based catalysts are the most commonly used catalysts in the traditional methane reforming field, and thus, researchers first consider Ni-based oxygen carriers for CLR. The oxygen carrying capacity of the Ni-based oxygen carrier is excellent, but it faces severe carbon deposits, which could cause the H 2 /CO ratio to be much higher than 2. At the same time, Ni-based oxygen carriers can only use air as the oxidant, and cannot be used for chemical looping hydrogen generation. Ni-based oxygen carriers are more expensive and unfriendly to the environment, which is not conducive to further industrialization. Fe-based oxygen carriers have the advantages of a wide range of sources and are environmentally friendly. Currently, a considerable amount of work has been done on the testing and characterization of iron ore. However, Fe-based oxygen carriers have poor activity and are easy to sinter, which results in lower CO selectivity, and reduced Fe could accelerate the methane cracking reaction, resulting in serious carbon deposits.
Based on these requirements and problems, we can summarize the recent progress and challenges in the development of oxygen carriers. Previous studies have focused on solving the problems of reactivity, carbon deposition, sintering, and stability. Taking CH 4 as an example, the chemical bond between carbon and hydrogen atoms in CH 4 is a stable sigma bond, and its chemical properties are relatively inactive. Therefore, CH 4 can participate in fewer reactions than other organic compounds. As a consequence, the high activity of the oxygen carrier is essential for the CLR of CH 4 . The reactivity of oxygen carriers generally rests on two parts, one is the theoretical conversion of fuel, and the other is oxygen transport and reaction kinetics. The theoretical conversion rate is mainly determined by the thermodynamic properties of the oxygen carrier. The transport and reaction kinetics are determined by the composition, structure, and texture properties of the oxygen carrier. The texture characteristics include pore volume, specific surface area, and porosity.
Ni-based and copper-based oxygen carriers have good reactivity to raw materials such as CH 4 , but the activities of Fe-, Mn-, Co, and Ce-based oxygen carriers are relatively poor. The addition of promoters or supports is considered to contribute to the improvement of activity. For example, the performance of iron oxide doped with 1% La is significantly improved compared with that of pure iron oxide [146]. Three-dimensionally ordered macroporous (3DOM) structures have been widely used in gas-solid reactions because of their uniform pore size (> 50 nm) and well-defined periodic structure, which could facilitate the adsorption and diffusion of reactant molecules. Compared with the nonporous CeO 2 -ZrO 2 oxygen carrier, the CH 4 conversion of oxygen carriers with different pore sizes can be increased up to approximately 3.6 times, and the H 2 production rate in the water splitting stage is also increased by 50% thanks to the relatively higher specific surface area, higher concentration of oxygen vacancies, and stronger oxygen mobility [158].
The generation of carbon deposits is one of the most commonly discussed difficulties in reforming catalysts. Taking methane reforming as an example, in the traditional methane reforming field, carbon deposition is mainly considered to be generated by methane cracking, and disproportionation reactions, which are also applicable to the chemical looping process. In the methane reduction stage, the Ni simple substance in the Ni-based oxygen carrier is reduced, which could quickly accelerate carbon deposition. Generally, for Ni-based oxygen carriers, CO 2 or H 2 O is added during the methane reduction stage to suppress carbon deposition or promote carbon deposition elimination. When Ni-based catalysts are used in chemical looping steam reforming, the TPO profiles of the spent Ni catalysts exhibit two CO 2 peaks, which means that there are two types of carbon deposits, one is probably absorbed CH x or oligomeric carbon that oxidizes at low temperatures (300 °C), and the other is polymeric carbon that oxidizes at higher temperatures. The amount of these two types of carbon deposits has a great relationship with the type of supports [159].
Different from Ni-based oxygen carriers, Fe-based oxygen carriers can be used in chemical looping methane dry reforming and water splitting. The carbon deposits produced during the methane reduction stage can use CO 2 as an oxidant to obtain CO during the oxidation stage. However, the existence of obvious carbon deposits could also affect the proportion of syngas in the methane reduction stage and the activity of the catalyst. At the same time, the generation of carbon deposits also affects its application in chemical looping hydrogen generation and the purity of H 2 in the steam oxidation stage. For Fe-based oxygen carriers, it is generally believed that CH 4 is first adsorbed on the surface of the oxygen carrier, and then activated for dehydrogenation. Next, it is oxidized to CO 2 by oxygen with a strong oxidizing capacity and to CO by oxygen with a moderate oxidizing capacity in the oxygen carrier. With the consumption of lattice oxygen, the supply rate or transmission rate of lattice oxygen cannot match the methane cracking rate, so carbon deposits are generated [160]. The cracking reaction of CH 4 on the surface of the Fe-based oxygen carrier starts as active phase Fe or Fe 3 C formed. Meanwhile, the increase in temperature and CH 4 concentration could promote the reduction of Fe-based oxygen, which indirectly promotes the production of carbon deposits.
In addition, the sintering of catalysts under high-temperature reaction conditions is a problem worthy of attention. The changes caused by carbon deposits could be reversible, while sintering is generally irreversible. It can be known through DFT calculations that the CH 4 adsorption energies and CO formation barriers are related to the particle size [130]. Therefore, with the sintering of the oxygen carrier, the particle size becomes larger so that the performance of the oxygen carrier changes significantly. The sintering of the catalyst inevitably affects the lattice oxygen transport rate, which causes the accumulation of carbon deposits. Suppression of catalyst sintering can be achieved by the confinement effects, that is, the use of nanostructures with specific morphology (3DOM, hydrotalcite and SBA-15 structure) to disperse the supported metal particles, thereby significantly improving the anti-sintering performance of the catalyst.
Improving the sintering resistance of the catalyst can also be achieved by adopting supports with large specific surface area or optimizing the preparation method. For copper-based oxygen carriers, the melting point of copper oxide is relatively low, so the sintering problem is a major problem in its development. The CuO/CuAl 2 O 4 oxygen carrier prepared by the sol-gel method maintained the porous structure, indicating that the sintering could be controlled [161]. The performance of different oxygen carriers applied in the CLR is summarized in Table 3.

Nickel based oxygen carrier
Compared with noble metal catalysts, Ni-based catalysts can exhibit excellent activity while being inexpensive, so they have been widely used and industrialized in methane steam reforming and dry reforming processes, and have achieved industrialization. With the advent and continuous development of CLR, Ni-based oxygen carriers have also been extensively studied. The supported NiO usually easily loses oxygen and exists in the form of metallic Ni while achieving catalytic function. It is well known that when the temperature is higher than the Hüttig temperature or near the Taman temperature, the sintering rate of metals and metal oxides will be accelerated [207], so the thermal stability of the oxygen carrier can be roughly estimated by these two temperatures. According to the melting point of Ni, the Tammann temperature and Hüttig temperature of metallic Ni are approximately 863 K and 518 K, respectively. However, the temperature of chemical looping steam reforming is usually higher than 923 K, so sintering will always occur during the process. Particle size is an important factor affecting the activity and stability of Ni-based catalysts, so various methods have been used to suppress sintering, thereby weakening the growth of particle size [208].
To improve the sintering resistance of Ni-based oxygen carriers, the first thing that comes to mind is to add structural promoters with a higher Taman temperature and better thermal stability, such as Al 2 O 3 [91,159,209,210], ZrO 2 [159,210,211], TiO 2 [159], SiO 2 [159,212], and MgAl 2 O 4 [137]. Such structural promoters provide a large surface area, which can play a positive role in dispersing Ni particles. At the same time, the interaction between Ni particles and the support also inhibits the migration of Ni particles on its surface, thus exerting anti-sintering effects. For example, Lasa

Review
Discover Chemical Engineering (2022) 2:5 | https://doi.org/10.1007/s43938-022-00012-3  et al. [209] introduced an Al 2 O 3 support for NiO-based oxygen carriers and found that the size of Ni particles stabilized at approximately 50 nm after several cycles, proving that no significant sintering occurred in the extended redox process. Temperature-programmed reduction (TPR) results showed that the interaction between Ni particles and the Al 2 O 3 support decreased with increasing Ni loading. In the mean time, Adánez et al. [213] suppressed the sintering of oxygen carriers by changing the types of Al 2 O 3 and the preparation methods. The specific surface area of the Ni-based oxygen carrier prepared by using γ-Al 2 O 3 and the incipient wet impregnation method after a 50-h test decreased by 65%, while the oxygen carrier adopting the α-Al 2 O 3 support and hot incipient wet impregnation method remained substantially unchanged after 100 h of testing [213]. When using Al 2 O 3 as the support, the appearance of NiAl 2 O 4 spinel is inevitable. Although NiAl 2 O 4 spinel may weaken the sintering of Ni particles, its oxygen carrying capacity and reaction performance are poor compared to NiO. Therefore, NiAl 2 O 4 [214,215] and MgAl 2 O 4 [216,217] spinels could be directly used as support to suppress the formation of NiAl 2 O 4 spinel. DFT calculations showed that the adsorption energy of Ni particles on the surface of ZrO 2 is − 4.89 eV and that the oxygen in NiO could bond with Zr atoms on the surface of ZrO 2 , which meant that NiO could be easily attached to the surface of ZrO 2 , forming a stable oxygen carrier [218]. The E vac of the Ni-Zr oxygen carrier was also calculated at 2.94 eV, and the oxygen carrier activity of ZrO 2 as a support was better than that of the MgAl 2 O 4 spinel support.
The SBA-16 is also applied to Ni-based oxygen carriers [131]. In order to improve the performance of chemical looping steam methane reforming, Rahimpour et al. [131,[219][220][221] carried out a series of studies on the application of Ni/SBA-16 oxygen carriers in chemical looping steam methane reforming, and conducted in-depth discussions on the properties of Ni/SBA-16 oxygen carriers and their modification by Ce and Y. With SBA as the support and the addition of Ce as the promoter, the performance of chemical looping steam methane reforming was significantly improved. The confinement effect of SBA and the interaction between Ce and Ni ensured the high dispersion of Ni, while the presence of Ce also stabilized the stability of the SBA skeleton.
The dispersibility of Ni in the supported oxygen carriers varies with the Ni precursor and the preparation method. Therefore, adjusting the type of Ni precursor and preparation method is another strategy method for improving sintering resistance [4]. A layered double hydroxide (LDH) precursor with a specific surface area (60.0 m 2 /g) was used to prepare a Ni-Mg-Al-O oxygen carrier, which promoted the dispersion of cations. BET and SEM results showed that the oxygen carrier remained porous after 100 cycles, which proved that its sintering was significantly suppressed. In addition, the addition of Mg formed a solid solution with Ni, and would also inhibit sintering to a certain extent [222].
For supported NiO-based oxygen carriers, sintering and carbon deposition are the main causes of deactivation. However, for NiFe 2 O 4 , it is possible that surface sintering is not the main cause of deactivation. The deactivation of NiFe 2 O 4 is more likely due to phase segregation or further sintering due to phase segregation, which aggravates the deactivation. Ma et al. [223] found that different phases, such as Ni and Fe 3 O 4 , appeared during the reduction of NiFe 2 O 4 . As the oxygen carrier was further reduced, FeO and NiFe phases appeared and an Fe-enriched needle-like structure was formed on the surface of NiFe 2 O 4 after the first cycle. And the phase segregation and deactivation became more serious after that. Ma et al. [224] introduced the CeO 2 into the NiFe 2 O 4 oxygen carrier to effectively alleviate the phase segregation problem. It was shown that the oxygen vacancy in CeO 2 promoted the mobility of lattice oxygen and thus prevented the phase segregation.
The stability of CH 4 keeps the reaction temperature at a high level, while reactants (ethanol and glycerol) need a lower reaction temperature. Dou et al. [89-91, 162, 225-228] carried out a series of works on the application of nickel-based oxygen carriers in ethanol or glycerol reforming. When Al 2 O 3 was used as the support, the CLR had higher glycerol conversion and H 2 yield than conventional reforming [91]. When nickel oxide was supported on montmorillonite, the cation exchange capability and confinement effect of montmorillonite promoted the dispersion of nickel, thereby improving the sintering and coking resistance of the oxygen carrier [90]. At the same time, Dou et al. [227] applied perovskite to CLR, and found that nickel can reversibly pass in and out of the perovskite structure during the process, thereby effectively suppressing the sintering of nickel particles. The addition of calcium and lanthanum promoters effectively increased the reactivity and stability of the oxygen carrier.
The high activity of nickel-based oxygen carriers makes the subsequent carbon deposition problem an obstacle to its development, so it is necessary to better understand the existence of carbon deposition and the corresponding solutions. The morphology or reactivity of carbon deposits in the reforming reaction depends on the specific reaction conditions and the structure of the oxygen carrier. According to the morphology of carbon deposits in previous literature, they can be generally classified into coated carbon and filamentous carbon [229]. They can be further divided into α-carbon (C α ), β-carbon (C β ) corresponding to steaming reforming [230] and α-carbon (C α ), β-carbon (C β ), and γ-carbon (C γ ) corresponding to dry reforming [231] according to the reactivity of carbon deposits.

3
C α can be oxidized by CO 2 , which is considered to be the carbon deposit that is easier to continue to participate in the reaction to generate CO. C β and C γ are the types of carbon deposits that are more difficult to participate in the reaction. C β may be gradually accumulated and transformed from C α in the course of the reaction, and C γ is graphite-like carbon species. C β and C γ are generally considered to be the causes of the deactivation of Ni-based catalysts in steam reforming and dry reforming, respectively. Some of the carbon deposits formed on the catalyst surface dissolve in Ni, and the remaining parts remain on the surface. The carbon deposits on the surface contain an orderly structure through dehydrogenation, surface migration and growth, which could encapsulate Ni and cause deactivation. Therefore, it is reasonably inferred that the evolution of the carbon deposit of the Ni-based catalyst, i.e., the initial C α formation and gradual accumulation of C α due to gasification imbalance and then transformation to poorly reactive C β , causes its deactivation gradually.
Specifically, for the oxygen carrier, the reason for carbon deposition is that the Ni particle size is too large, or there are acid sites or carbon deposition nucleation centers on the surface. A large number of studies have been carried out on the causes of carbon accumulation. Certain strategies for enhancing coke resistance in traditional methane reforming are suitable for CLR, but some methods, such as adding additives that enhance O 2 or CO 2 adsorption, might not be suitable for CLR. Highly dispersed Ni nanoparticles with small particle sizes exhibit excellent coke resistance because the Ni particles are small enough to prevent the carbon nanofibers from nucleating on them, and carbon nucleation at the step edges and subsequent growth are also suppressed [232]. Hence, the abovementioned method for improving the dispersion of Ni particles can not only improve the anti-sintering ability of the oxygen carrier but also effectively alleviate the carbon deposition problem of the oxygen carrier.
Immobilizing Ni ions in a stable structure such as perovskite is also a strategy to weaken carbon deposition, as perovskite structures have good oxygen migration capacity and can balance the rate of carbon generation and elimination to a better extent. However, the aggregation of perovskite oxygen carriers during calcination results in their small specific surface area, which limits their application. Li et al. [164] loaded LaNiO 3 on the montmorillonite (MMT) support, integrating the strong oxygen migration ability of perovskite with the large specific surface area of MMT. Compared with the unsupported perovskite, LaNiO 3 /MMT particles had a smaller particle size, and the particle size was mainly distributed between 10 and 20 nm. In the ethanol reforming cyclic test, the activity of LaNiO 3 /MMT after 10 cycles only decreased by 12.4%, which was much lower than that of LaNiO 3 .
Metcalfe et al. [163] prepared the Ni-containing perovskite oxygen carrier and controlled the exsolution of nickel particles to optimize the reaction process (Fig. 10). By reduction under hydrogen, an oxygen carrier (Ni-rABO 3 ) having nickel particles on the surface and within the bulk phase could be obtained. The particle size of the surface particles was larger than that of the bulk particles, and the proportion of the bulk particles was higher. By changing the temperature and treatment time of the oxygen carrier, it was found that the interparticle distance and size of the particles were correspondingly changed. At the same time, the proportion of the bulk particles and the corresponding oxygen capacity increased with increasing treatment time or temperature. For more intuitive analysis, Metcalfe et al. [163] fitted the oxygen uptake measurement with a logistic law and plotted the corresponding oxygen capacity (ζ G , mol O per mol perovskite) and time constant of oxygen exchange (τ, h −1 ) in Fig. 10b. It was found that the ζ G was directly proportional to the bulk nickel content (Ni B , wt.%), and τ was related to the ratio of the average bulk particle diameter (s, nm) to the average distance between neighboring bulk particles (d, nm).
In order to prove the superiority of Ni-rABO 3 , Ni-rABO 3 and Ni/Al 2 O 3 were applied to the methane reforming reaction. Ni/Al 2 O 3 showed low selectivity for partial oxidation products and high carbon deposition selectivity. In contrast, Ni-rABO 3 exhibited excellent selectivity for partial oxidation products with little carbon deposition. To further prove the importance of the coexistence of surface and bulk particles, samples with only surface or bulk particles were tested and found to be inactive. The operando analysis of oxygen carriers was used to study the mechanism of bulk phases and surface particles (Fig. 10c). When the temperature was approximately 550 °C, CH 4 started to be consumed, corresponding to the reduction of surface nickel oxide particles. Next, the bulk nickel oxide was reduced, and as the bulk nickel oxide was depleted, the perovskite was reduced. The method of obtaining bulk and surface particles through reduction treatment provided important guidance for the development of nickel-based oxygen carriers and perovskite structures.
In addition, the selectivity and anti-carbon capacity of oxygen carriers are also influenced by the properties of the particle. In CLR, support with good oxygen carrying capacity and oxygen mobility can be selected to provide oxygen for the reaction process of Ni particles while supporting. CeO 2 is added to the Ni-based oxygen carrier due to its good sintering resistance and excellent oxygen mobility [165,167,233,234].
In addition to eliminating carbon deposits, chemical looping can be used to utilize the activity of Ni-based oxygen carriers to enable the production of H 2 and CO. Tian et al. [235] achieved H 2 and CO production by passing biogas into the reaction tube containing two catalyst sections. First, in the H 2 production stage, calcium oxide absorbs CO 2 from the feedstock to produce calcium carbonate, followed by the cracking of methane by the Ni-based oxygen carrier, which produces carbon deposition on the Ni-based oxygen carrier. Then, in the CO production stage, the calcium carbonate in the reaction tube decomposes to produce CO 2 , followed by the reaction of carbon on the Ni-based oxygen carrier at the lower end with CO 2 to produce CO. Wang et al. [236] achieved the preparation of H 2 and CO through Ni/La 2 O 3 carriers. The H 2 preparation was achieved using the methane cracking ability of Ni, while the carbon accumulation on the catalyst surface reacted with the incoming CO 2 to achieve CO production. These two processes utilize the methane cracking ability of nickel-based catalysts to achieve efficient preparation of H 2 and CO, providing a new idea for the development of nickel-based oxygen carriers.

Iron based oxygen carrier
Iron is the most commonly used transition metal and the second most abundant metal in the earth's crust. The outer electron configuration of Fe is arranged as 3d64s2 so that it has + 3, + 2, and zero valence. Because of the different oxidizing abilities displayed during the transition between different valence states of iron oxide and the excellent water or CO 2 dissociation ability of metallic Fe, Fe-based oxygen carriers have been applied in various chemical looping processes with different target products. Because of the various advantages exhibited by Fe-based oxygen carriers, it is a promising candidate for the industrialization of chemical looping processes. Fe-based oxygen carriers can be generally divided into two categories, namely, synthetic Fe-based oxygen carriers and naturally occurring iron ore-based oxygen carriers. The application of pure iron oxide to the chemical looping process has been previously investigated [237]. Trevisanut et al. [238] applied Fe 3 O 4 to chemical looping hydrogen generation and found that the carbon content of the oxygen carrier was controlled to 1% after 20 cycles. However, during the reaction process, iron oxide may be reduced by bioethanol into unstable iron carbide, which can be decomposed into Fe Fig. 10 a 3D model of an oxygen carrier particle with nanoparticles dispersed on its surface and within its bulk. b Parallel axes plot for the samples reduced at 900 °C for 0 h (dark grey), 10 h (dark blue) and 30 h (blue) and at 1000 °C for 10 h (light blue). c XRD data acquired during the TPR under 5% CH 4 of a system with submerged nanoparticles presented as 2D plot, as a function of diffraction angle, time and corresponding temperature; d CH 4 consumed and corresponding products produced during the experiment described in c. e NiO content and perovskite unit cell parameter calculated from c. f Schematic of CH 4 conversion mechanism corresponding to the main stages identified from c. Reproduced from ref. [163] with permission from John Wiley and Sons, copyright 2020 and carbon, thus promoting the generation and accumulation of carbon deposits with increasing cycle numbers of the redox cycles. Ma et al. [239] studied the morphology and structural changes of iron oxide during the chemical looping reaction. After multiple cycles, it can be found that the surface of the oxygen carrier was sintered and reduced due to the instability of the iron oxide during its conversion. At the same time, the mechanical integrity and strength were decreased due to the continuous migration of Fe ions. Zheng et al. [240] compared the performance of iron oxide and nickel-impregnated iron oxide oxygenate carriers. The CH 4 conversion and H 2 yield of iron oxide alone were low, while the Ni-impregnated oxygen carriers had high H 2 yield, which may be due to the synergistic effect between nickel and iron. The nickel on the surface of the oxygen carrier provides catalytic sites while the iron provides lattice oxygen, which promotes H 2 production. Kidambi et al. [241] prepared Al 2 O 3 -supported iron oxide oxygen carriers with different Fe 2 O 3 loadings. The particle size of iron oxide was found to decrease with the reducing loading of iron oxide, and the particle size of iron oxide with a loading of 100% was 3.3 times larger than that of iron oxide with a loading of 50%.
As mentioned in the section of primary material selection, the performance of the supported iron oxide oxygen carriers is closely related to the particle size of the iron oxide, so it is particularly important to obtain iron oxide particles with a small particle size. High dispersion of iron oxide particles can be achieved by using the SBA-15 support via the confinement effect. Fan et al. [130] successfully synthesized SBA-15 supported iron oxide with high dispersion (Fig. 11). The particle sizes of iron oxide particles confined within SBA-15 (Fe 2 O 3 @SBA-15) and unsupported iron oxide particles were between 3-5 nm and 50-100 nm, respectively. After redox cycles, the particle size of the Fe 2 O 3 @SBA-15 oxygen carrier increased by 5-8 nm, while the particle diameter of the unsupported Fe 2 O 3 was between 1 and 10 μm. DFT calculations showed that the CH 4 adsorption energies and CO formation barriers were related to the particle size. The Fe 2 O 3 @SBA-15 oxygen carrier achieved nearly 100% CO selectivity at low temperatures, and the conversion rate was approximately 1.69 times than that of unsupported Fe 2 O 3 . Since the oxygen transmission rate and the subsequent reaction performance are also closely related to the particle size, iron oxide is generally supported on a support or restricted in a composite oxide. Therefore, synthetic Fe-based oxygen carriers are mainly divided into supported and composite oxide oxygen carriers. The metal dispersion degree and anti-sintering capacity were the two most concerned factors for supported oxygen carriers, and strategies like changing the supports and dopants were employed to conduct surface or bulk phase modification. For composite oxide oxygen carriers, taking perovskite as an example, the performance can be optimized by replacing the metal at the A and B sites. The natural ore oxygen carriers are mainly hematite and ilmenite [242]. Natural ore generally needs to be calcined at high temperature before being applied to the chemical looping process. Although the main component of the ore is Febased oxides, the properties of ores may vary due to changes in other components caused by different ore origins [242].
For supported oxygen carriers, the most commonly used supports are SiO 2 and Al 2 O 3 . SiO 2 has a poor dispersion effect on iron oxide during the reaction process, and reacts irreversibly with iron oxide to form iron silicate, so it is less commonly used [243]. Al 2 O 3 as a support can better disperse iron oxide and improve the sintering resistance of the oxygen carrier [244]. Fe 2 O 3 /Al 2 O 3 oxygen carriers have been widely used in chemical looping methane reforming and alcohol reforming. Kang et al. [174] used the Fe 2 O 3 /Al 2 O 3 oxygen carrier in the chemical looping dry reforming process. In the 20 cycles test at 900 °C, the CH 4 conversion and the CO selectivity were all above 95% and remained stable. Meanwhile, the H 2 /CO ratio of the oxygen carrier was approximately 2.2, indicating that the carbon deposition was not significant. Qin et al. [245] successfully applied Fe 2 O 3 /Al 2 O 3 oxygen carriers in chemical looping reforming of ethanol-containing organic wastewater. When the ethanol concentration was 5% and the reaction temperature was 800 °C, the carbon conversion and syngas yield of the oxygen carrier were 100% and 3.325 L/g, respectively. However, it was found in the experiment that Al 2 O 3 went through a solid phase reaction with Fe 2 O 3 during the cycle to produce spinel. The effect of FeAl 2 O 4 spinel is contradictory because its formation can reduce the sintering of oxygen carriers while reducing the storage capacity of Fe 2 O 3 [246]. Yüzbasi et al. [247] prepared Al 2 O 3 -supported iron oxide oxygen carriers with a loading of 80% by the sol-gel method and used three different Fe salts as Fe precursors. XRD characterization revealed that the FeAl 2 O 4 spinel only existed in the oxygen carrier using ferric chloride as a precursor. In addition, although the oxygen carrier using ferric chloride as a precursor possessed no advantage compared with the other two precursors in the performance test, its performance remained stable in 15 cycles. Compared to the other two oxygen carriers, this oxygen carrier had the largest proportion of spinel, which played a role in preventing the oxygen carrier from sintering during the reaction, thus leading to its good stability.
The existence of FeAl 2 O 4 spinel is more significant for CLC. First, in thermodynamics, when Fe 2 O 3 reacts with CH 4 at 900 °C to produce Fe 2+ , CO 2 , and H 2 O, the Gibbs free energy of Fe 2 O 3 to FeAl 2 O 4 is 1.5 times less than that of Fe 2 O 3 to FeO, suggesting that the addition of Al 2 O 3 thermally results in more oxygen conversion in CLC. Second, it is currently believed that only Fe 2 O 3 to Fe 3 O 4 produces high purity CO 2 . According to the thermodynamic calculation by HSC chemistry software, it can be known that at 900 °C, the addition of Al 2 O 3 causes the oxidation products to have an impact on the reduction of Fe 3 O 4 by CH 4 to FeO, making it more inclined to produce CO 2 . Finally, the presence of FeAl 2 O 4 spinel also means that Fe 2 O 3 is well dispersed on Al 2 O 3 because the reduction of specific surface area caused by sintering could prevent Fe 2 O 3 and Al 2 O 3 from contacting closely, thus significantly reducing the amount of spinel produced in the reduction process. Wang et al. [248] added different proportions of silicon to the Al 2 O 3 support to enhance the sintering resistance of the oxygen carrier. XRD characterization showed that the presence of silica inhibited the conversion of γ-Al 2 O 3 to α-Al 2 O 3 to ensure the stability of the specific surface area, and a large amount of FeAl 2 O 4 spinel was produced during the reduction process. The best-performing sample decreased its oxygen transfer capacity by only 6% after sixty cycles, indicating that it had good cycle stability. However, in the process of chemical looping hydrogen generation or dry reforming, the oxidation ability of water or CO 2 was thermodynamically not strong enough to oxidize the Fe 2+ in FeAl 2 O 4 spinel back to Fe 3+ , which meant that the yield of CO or H 2 was decreased.
The formation of FeAl 2 O 4 spinel can be prevented by the rational design of oxygen carriers. Hafizi et al. [249] added 5% Mg to the Al 2 O 3 -supported iron oxide oxygen carrier, where the presence of MgAl 2 O 4 spinel could be found in the prepared oxygen carrier without the presence of FeAl 2 O 4 spinel. Meanwhile, the proportion of FeAl 2 O 4 spinel in the oxygen carrier after 15 cycles decreased significantly. In addition to suppressing the formation of spinel by adding Mg, Mg-Al spinel support can also be used directly [138,140,243]. In order to maximize the production of CO, Buelens et al. [139] developed a super-dry reforming method, which adopted Fe 2 O 3 /MgAl 2 O 4 as an oxygen carrier, Ni/MgAl 2 O 4 as a reforming catalyst, and CaO/Al 2 O 3 as a CO 2 sorbent. Unlike other chemical looping processes that directly pass O 2 , H 2 O or CO 2 to oxidize the oxygen carriers, this process used CaO/Al 2 O 3 to achieve the storage of CO 2 in the reduction stage 1 3 and released CO 2 to oxidize the oxygen carrier in the oxidation stage. The yield of CO is also maximized while achieving the in situ removal of CO 2 . Through long-term cycle tests, it was found that the Fe 2 O 3 /MgAl 2 O 4 oxygen carrier possessed good cycle stability and obtained a high space-time yield of CO. Yttrium was also added to Al 2 O 3 -loaded iron oxide to form a uniform garnet structure with Fe and Al when the ratio of Y 2 O 3 to Fe 2 O 3 was 1.5 [176]. Moreover, according to the [57] Fe Mössbauer spectra, it was found that the sintering was significantly alleviated with the addition of Y because iron oxide with low amount of yttrium doping had a smaller particle size than that without doping. With the increase of doping amount and the activation of oxygen carriers, more Fe 3+ was found to enter the garnet structure. The CO production of the oxygen carrier also improved with increasing doping amount. On the basis of the DFT calculation, the reason why the garnet structure was highly selective for CO was that the E vac of the oxygen carrier doped with yttrium was approximately 41% higher than that of the non-doped oxygen carrier. Fe 2 O 3 /Al 2 O 3 oxygen carriers also face problems (carbon deposition, sintering, and poor reactivity) during the CLR process. The addition of metallic Ni can effectively alleviate the problem of poor reactivity of iron oxide oxygen carriers. Huang et al. [168] added an equal proportion of NiO to the Fe 2 O 3 /Al 2 O 3 oxygen carrier, and found that the conversion of CH 4 is up to 3.75 times higher than that of the pure iron oxide oxygen carrier, and the CO 2 selectivity was also reduced by 81%. Kang et al. [174] also obtained the Ni-entrapped Fe 2 O 3 /Al 2 O 3 oxygen carrier by the sol-gel method. The addition of 1% Ni increased the interaction between the metal and the support, which significantly improved the CO selectivity and reduced the H 2 /CO ratio. There were two main origins of carbon deposition on the Fe 2 O 3 /Al 2 O 3 oxygen carrier, one was that the limited oxygen transport capacity and oxygen migration capacity of iron oxide could not remove carbon deposition in time and the other was that Al 2 O 3 was an acidic support, which promoted the generation of carbon deposition. Therefore, the elimination of carbon deposition is considered from these two aspects. Carbon deposition due to the acidity of the support was mitigated by adding a certain proportion of alkali metals. Through DFT calculations, Feng et al. [250] found that lithium, sodium, and potassium alkali metals tended to stay on the surface of the oxygen carrier. Because alkali metal owned a lower valence state than Fe, the introduction of alkali metal lowered the E vac on the surface, making oxygen carriers more active. Zhu et al. [144] added K 2 CO 3 to the Fe 2 O 3 /Al 2 O 3 oxygen carrier and applied it to chemical looping hydrogen generation. Performance tests showed that the K 2 CO 3 -doped Fe 2 O 3 /Al 2 O 3 oxygen carrier did not show significant carbon deposits at a CH 4 concentration of 40% and remained stable, while carbon deposits of the undoped Fe 2 O 3 /Al 2 O 3 oxygen carrier increased significantly over time. The purity of H 2 in the steam oxidation stage was also improved due to the addition of K 2 CO 3 . CeO 2 with good oxygen migration ability and oxygen storage ability was also added to the Fe 2 O 3 /Al 2 O 3 oxygen carrier to inhibit the formation of carbon deposits. CeAlO 3 , Al 3 Fe 5 O 12 , and AlFeO 3 were formed by adding 5% CeO 2 to the iron oxide oxygen carrier through the sol-gel method, and CeAlO 3 activated and decomposed CO 2 , thereby providing active surface oxygen for carbon deposition elimination [145]. At the same time, the addition of CeO 2 generated more oxygen vacancies to promote the transport of lattice oxygen. The thermogravimetric analyzer test suggested that the coke-resistant ability of the CeO 2 -doped Fe 2 O 3 /Al 2 O 3 oxygen carrier was enhanced. Meanwhile, in the fixed-bed test, the purities of H 2 and carbon-containing substances in the steam oxidation stage were 100% and 0, respectively, which proved that no carbon deposit was generated in the reduction stage. Kang et al. [177] prepared the ceria-enhanced Fe 2 O 3 /Al 2 O 3 mesoporous oxygen carrier with a large specific surface area and used it for chemical looping dry reforming. Due to the large specific surface area, the reaction gas was in close contact with CeO 2 . Therefore, compared with the Fe 2 O 3 /Al 2 O 3 oxygen carrier prepared by the wetness impregnation method, the H 2 /CO ratio and average carbon deposit decreased by 28% and 63%, respectively. In the preparation of catalysts, inert carriers are mostly used, and oxygen carriers are no exception. However, Zeng et al. [251] believed that the addition of Al 2 O 3 and other inert materials diluted the active components, which made carbon deposition and other problems more serious, and that the addition of ion-conducting supports promoted the transport of oxygen from the bulk phase to the surface. Indeed, the addition of the gadolinium-doped cerium oxides (GDC) support allowed the oxygen carrier to achieve maximum conversion at a lower temperature and in a shorter time than pure Fe 2 O 3 and Fe 2 O 3 /Al 2 O 3 . Zeng et al. [252] conducted long-cycle tests on Fe 2 O 3 /Gd 0.3 Ce 1.7 O 2−δ and found that the oxygen carrier maintained good activity for 30 cycles. Also, it was shown that oxygen ion conductivity is the rate-determining step of the process. Therefore, the introduction of Gd 0.3 Ce 1.7 O 2−δ support enhanced the oxygen ion conductivity of the oxygen carrier, which is the reason for the good reactivity of the oxygen carrier.
During the CLC process, the addition of La 2 O 3 can significantly inhibit the phase separation of the iron oxide oxygen carrier, which makes the oxygen carrier show good reactivity and stability. Tang et al. [180] combined the advantages of La 2 O 3 and CeO 2 and added them together to the iron oxide oxygen carrier. XRD characterization showed that LaFeO 3 and CeFeO 3 formed during the reaction process and that the dispersion of iron oxide was improved due to the addition of La and Ce. The formation of LaFeO 3 perovskite enabled lattice oxygen to be quickly transferred from the bulk phase to the surface, while the formation of CeFeO 3 allowed more oxygen vacancies in the oxygen carrier, thus increasing the oxygen migration capacity. Through the cycling test, it was found that although the Fe 2 O 3 /Al 2 O 3 carrier possessed the highest CO selectivity in the first cycle, it rapidly decreased, and the carbon deposition increased significantly. For the oxygen carrier doped with La, it maintained good stability in 10 cycles, which proved that the addition of La increased the stability of the oxygen carrier. When CeO 2 or Zr/La-modified CeO 2 was used as a support for an Fe-based oxygen carrier, the oxygen carrier exhibited good chemical looping performance [253][254][255]. When Zr-doped CeO 2 was used as a support, no CO x was found in the steam oxidation stage in the chemical looping hydrogen generation, and the presence of Zr also prevented the migration of Fe ions, thereby improving the sintering resistance of the oxygen carrier [253]. Xiong et al. [256] further modified the CeO 2 support, thus contributing to the formation of oxygen vacancies in the carrier, which further affected the oxygen ion conductivity. Meanwhile, the introduction of lanthanum and gallium promoted the formation of oxygen vacancies and inhibited the outward migration of iron ions to a certain extent.
Researchers are more concerned about how the oxygen carrier changes during the chemical looping reforming process, so the advantages of in situ characterization in determining the reduction path become more prominent. Müller et al. [257] found that the reduction path of Fe 2 O 3 /ZrO 2 through in situ XANES and ex suit XRD was consistent with the existing literature. Fe 2 O 3 followed the path of Fe 3 O 4 , FeO and Fe, and the process from FeO to Fe was the slowest. Zhou et al. [258] also studied the reduction process and the effect of reduced Fe species in chemical looping dry reforming of methane. Similarly, Fe 2 O 3 was reduced to Fe 3 O 4 at the earlier stage of the reaction, converting CH 4 to CO 2 . However, the small amount of CO 2 would inhibit the subsequent partial oxidation of methane to syngas. Introduction of reduced catalyst with low Fe valent could increase syngas production and it seemed that these reduced pieces, e.g., Fe 0 , could consume CO 2 with its ability in catalysing the dry reforming, alleviating inhibition effect of CO 2 generated as result of full CH 4  Compared with the undoped one, the doping of Cu made the oxygen carrier complete reduction in fewer pulses, which proved that the addition of Cu changed the reduction path of the original oxygen carrier and obviously promoted the oxygen carrier. X-ray absorption spectroscopy (XAS) characterizations can not only judge the reduction path but also understand the atomic coordination environment and surface disorder degree of the oxygen carrier. Müller et al. [259] revealed the effect of pH on the preparation process more clearly with the aid of XAS characterizations. XANES results showed that pH could affect the local coordination environment of Fe atoms on the oxygen carrier, and the octahedral environment of iron atoms became more distorted as the pH decreased. At the same time, EXAFS characterization indicated that the degree of disorder on the surface also increased with decreasing pH. This high degree of disorder was attributed to the insertion of Fe 3+ into ZrO 2 .
In order to judge more intuitively the oxygen conductivity of the oxygen carrier and provide more direct evidence for oxygen ion conduction, electrochemical testing methods are introduced into the oxygen carrier characterization process to show the oxygen ion conductivity of the oxygen carrier [251,259]. Electrochemical impedance spectroscopy (EIS) and electrical conductivity relaxation (ECR) measurements are representative electrochemical tests that are commonly used in button batteries and solid oxide fuel cells, and can obtain the conductivity of the tested materials.
The addition of the support generally plays a role in dispersing the active components, but the ECR test shows its more important significance. The addition of ZrO 2 support to the Fe 2 O 3 oxygen carrier increased the conductivity of the oxygen carrier, and significantly reduced the activation energy of ion transport, meaning that ZrO 2 enhanced the solid diffusion of oxygen anions and electrons in the oxygen carrier [259]. For the EIS test of oxygen carriers, the conductivity can be divided into two parts, one is generated by oxygen ions and the other is generated by electrons. From the experimental results, compared with the conductivity of oxygen ions, the conductivity of electrons was negligible, indicating that the conductivity of oxide ions was dominant. Moreover, it was found that the addition of ion-conducting supports significantly increased the conductivity of oxygen carriers, providing theoretical support for the adoption of perovskite and GDC materials with good ion conduction [251]. In addition to revealing the role of the carrier, the ECR test is used to detect the effect of doping. Gong et al. [260] adopted ECR to obtain the oxygen bulk diffusion coefficient and surface exchange coefficient of the Ce-doped perovskite oxygen carrier, and found that the doping of cerium reduces the activation energy for lattice oxygen migration. In order to clarify the reason for the increase in conductivity caused by doping, Gong et al. [261] conducted an in-depth discussion and found that with the addition of Ce, the degree of distortion of the FeO 6 octahedral increased, which might be the reason for its conductivity change.
In order to understand the phase change of Fe 2 O 3 -La 0.7 Sr 0.3 FeO 3 during cycling, in situ XRD characterization was adopted. Ex situ XRD showed that the oxygen carrier was composed of La 0.7 Sr 0.3 FeO 3 and SrFe 12 O 19 before the reduction began [262]. At the beginning of the reduction, perovskite was found to shift to a low angle by in situ XRD, accompanied by the disappearance of SrFe 12 O 19 and the appearance of Fe. After several scans, the Ruddlesden-Popper (RP) structure also appeared, and finally, La 2 O 3 and a small amount of SrO appeared. After water oxidation, it was found that the initial state was not fully restored, which meant that the redox cycle was not completely reversible, and the composite material was in a dynamic change process. Multilength X-ray computed tomography (X-ray CT) was performed in order to observe the overall change in the oxygen carrier more intuitively. Therefore, the surface and phase images of the oxygen carrier were visually observed, and the phase and pore structure distribution of the oxygen carrier in the dynamic change process were also obtained from the images, which provided a possibility for better observation of the changes of the oxygen carrier in the cycling process.
Fe-based composite oxide oxygen carriers are oxygen carriers with specific structures, mainly including spinel ferrite, ilmenite, and perovskite. The effect of mechanical mixing of two metal oxides is often the sum of the activities of the individual metal oxides. The difference between composite oxides and mechanical mixing is that the added components can improve the catalyst's activity by stabilizing the catalyst structure, changing the catalyst electronic structure, and forming defects on the surface. At the same time, composite oxides are mostly nonstoichiometric compounds with defects in the crystal structure. Therefore, they exhibit excellent oxygen and electron transfer behaviors in oxidation-reduction reactions.
Spinel composite oxides have been used for a long time in the complete and selective oxidation of hydrocarbons because of their low cost, environmental friendliness, high temperature resistance, and stable chemical properties. Zeng et al. [263] prepared Co-Mn co-doped iron-based spinel oxygen carriers and applied the oxygen carriers to the chemical looping CO 2 splitting process. The test results showed that the Mn 0.2 Co 0.8 Fe 2 O 4 oxygen carrier exhibited the CO yield comparable to perovskite oxygen carriers at 650 °C, proving the feasibility of the spinel oxygen carrier application. Huang et al. [264] conducted a detailed exploration of the reaction mechanism of spinel oxygen carriers by in situ XPS. They found that the reaction process was all carried out on the surface of the oxygen carrier, so the concentration gradient drove the gradual transfer of lattice oxygen from the bulk phase to the surface. Evdou et al. [265] tested the performance of spinel ferrites with different A-sites in chemical looping, and found that the performance and stability of oxygen carriers change significantly with various A-site metals. The CuFe 2 O 4 oxygen carrier maintained stability while exhibiting the highest CH 4 reactivity and the largest amount of lattice oxygen involved in the reaction. Compared to CuFe 2 O 4 , the initial reactivities of NiFe 2 O 4 and ZnFe 2 O 4 were moderate, and their deactivation was obvious in five cycles, but the causes of Ni and Zn iron spinel deactivation were different. XRD characterization of the oxygen carriers after redox cycles showed that ZnFe 2 O 4 was decomposed into iron oxide and metallic Zn, while NiFe 2 O 4 showed no phase separation. There were aggregates of zinc in ZnFe 2 O 4 after cycling, and the NiFe 2 O 4 after cycling showed obvious sintering according to the SEM images. However, SEM-EDS showed that Ni and Fe simple substances of NiFe 2 O 4 were evenly distributed, and the ratio of Ni/Fe was 1/2, proving that the cause of deactivation was sintering rather than phase separation.
Solving phase separation and sintering issues is the focus of future research on spinel oxygen carriers. Huang et al. [266] investigated the application of NiFe 2 O 4 oxygen carrier in chemical looping hydrogen generation. Since Ni was thermodynamically impossible to decompose water, it was found in the TGA test that the H 2 production capacity gradually weakened with the addition of Ni. At the same time, it was found in fixed bed experiments that the H 2 production of Fe 2 O 3 and NiFe 2 O 4 decreased with decreasing reduction time, but spinel reached a deeper reduction degree than iron oxide in a short time due to its strong oxidation capability. Therefore, when the reduction time was shortened to 12 min, the H 2 yield of spinel exceeded that of iron oxide, illustrating that spinel was suitable for chemical looping hydrogen generation. However, Fe was separated in the form of iron oxide after a number of cycles, causing the spinel structure to be destroyed. Lee et al. [267] experimentally found that spinel-loaded oxygenates not only face the problem of phase separation, but also have the problems of surface grain aggregation and surface densification with the increasing number of cycles. These problems were effectively solved by introducing Al into the spinel to form a solid solution between the spinel and Al, which is beneficial for the long-term use of spinel oxygen carriers.
As mentioned earlier, NiFe 2 O 4 spinel faces sintering problems, so Al 2 O 3 is added to promote the dispersion of Ni and Fe to suppress sintering and phase separation. Compared with pure NiFe 2 O 4 spinel, the addition of Al 2 O 3 made only a small amount of iron oxide appear in the oxygen carrier after five cycles, and the H 2 yield remained stable for 20 cycles. The reason why Al 2 O 3 enhanced the anti-sintering ability was that its uniform distribution on the surface of the oxygen carrier made the direct contact of adjacent Ni-Fe particles difficult, thus increasing the stability. At the same time, although Ni was thermodynamically incapable of being oxidized by steam, the strong phase action of Fe-Ni in  [268] applied CeO 2 , ZrO 2 , and CeZrO 2 supports to NiFe 2 O 4 spinel oxygen carriers. When ZrO 2 and CeZrO 2 were used as supports, oxygen carriers suffered serious phase separation and sintering problems. However, the NiFe 2 O 4 /CeO 2 oxygen carrier improved the oxygen migration ability while maintaining good cycle stability without phase separation. Naturally occurring ilmenite has shown good performance in CLC. Fan et al. [269] applied it to CLR, and fully analyzed the morphological changes of ilmenite during the reaction. According to the SEM characterization results, the Ti-Fe composite oxide formed nanobelts on the surface after oxidation treatment at 700 °C, and the oxygen carrier became porous with increasing cycle number. The DFT calculation results showed that the formation of surface nanobelts mainly composed of iron oxide was due to the fact that the energy barrier of Fe ions migrating to the surface was smaller than that of Ti ions. At the same time, FeTiO 3 had a lower E vac than Fe 2 O 3 , which made it easier to form a porous structure on the surface after cycling. The porous structure of ilmenite worsened its mechanical properties, and the formation of nanobelts also promoted phase separation. In order to alleviate the problems of mechanical properties and phase separation of ilmenite, Fan et al. [143] adopted an Al-based skeleton to the preparation of oxygen carriers. The existence of the Al-based skeleton enabled the oxygen carrier to maintain good activity and stability under 3000 cycles.
Perovskite has gained prominence in three-way catalysis, complete oxidation of hydrocarbons, and fuel cells due to the variability of its constituent elements, valence states, stoichiometric ratios, and oxygen vacancies [270]. The defects in perovskite are mainly oxygen vacancies, which can not only promote the transport of lattice oxygen but also assist the activation of many reactions, so perovskite can be well applied in chemical looping. La-perovskite is the most widely used perovskite-type oxygen carrier in CLR. Mihai et al. [132] applied LaFeO 3 perovskite to chemical looping methane partial oxidation, and investigated the influence of the particle size and oxygen content of the oxygen carrier on the reaction process and kinetics. XRD characterization revealed that the particle size of the oxygen carrier changed with the complex agent selected during the preparation process, which in turn affected the cycling stability of the oxygen carrier. By analyzing the performance of the oxygen carrier, it was found that the recovery time for the oxygen carrier in the oxidation stage was much less than the reaction time in the reduction stage. Based on performance data, Mihai et al. [132] proposed that the types of methane oxidation products were closely related to the coordination environment of Fe, and the coordination environment changed dynamically during the redox process. During the reaction, the types of Fe could be roughly divided into three categories according to their coordination environment, and different types of iron correspond to different product distributions. For example, iron highly coordinated with oxygen atoms might be the active site responsible for complete oxidation, and iron with highly coordinated oxygen vacancies may be responsible for carbon deposition. UV-vis characterization showed that the absorption edge energy of the oxygen carrier with small particle size was larger, which meant a high resistance for O removal from the perovskite. Meanwhile, the method of controlling the surface oxygen concentration by controlling the oxidation time was adopted to optimize the performance. It was found that when the oxidation time was 95 s, almost pure syngas was obtained. However, due to incomplete oxidation, the H 2 /CO ratio and carbon deposition increased. Chen et al. [271] carried out a detailed study on the coordination environment of iron in perovskites. They found that the reduction process of the oxygen carrier is divided into three stages, and the coordination environment of iron in the perovskite is different in these three stages. And the coordination environment of iron, that is, the concentration of oxygen vacancies, changes the energy barrier for complete oxidation of methane. Therefore, the transition of the oxygen carrier from an oxygen-rich surface to a surface dominated by oxygen vacancies implies a transition from complete oxidation of methane to selective oxidation.
For perovskites used in the chemical looping process, it is generally to use different metals to replace the A or B positions. According to the principle of electrical neutrality, perovskites formed by replacing similar A or B ions with similar ions can not only change the original oxidation state and coordination state of A or B but also cause defects in the structure, especially the concentration of oxygen vacancies, to change significantly. For LaFeO 3 perovskite, the modification of the A-site mainly uses Sr or Ce, while the modification of the B-site mainly uses transition metal elements. He et al. [118] replaced the A and B sites of LaFeO 3 perovskite, and found that when a part of La was replaced by Sr, the oxygen vacancies of the oxygen carrier were increased and the decomposition of CH 4 was suppressed, so the performance of the oxygen carrier was significantly improved. When 30% of Fe was replaced by Co, the oxygen-donation ability, anticoking performance, and H 2 generation capacity of the oxygen carrier were all improved, and it remained stable for 20 cycles [116]. Introduced Ni species in LaNi 0.07 Fe 0.93 O 3-x were well dispersed on the surface of LaFeO 3 and could play a catalytic role in adsorbing and activating CH 4 during the reduction process as revealed through experimental investigation and DFT calculations, resulting in enhanced activity and lowered reaction temperature for syngas and H 2 generation. The reduced Ni species generated in the reduction step could also promote the splitting of H 2 O to H 2 at relatively low 1 3 temperatures. The formation of H 2 started at 302 ℃, which was about 70 ℃ lower than that of reduced pure LaFeO 3 and the improved performance was able to remain after 50 successive redox cycles [272]. Li et al. [273] adopted Ce and Ni to dope the A-and B-site of LaFeO 3 perovskite, respectively, and investigated the effect of calcination temperature on the reaction performance of the oxygen carriers. The experimental results showed that with the increase of the calcination temperature, the nickel gradually migrated to the surface of the oxygen carrier, thus making the oxygen carrier more prone to carbon accumulation, so that the low calcination temperature may be more favorable for the LaFeO 3 perovskite to improve the anti-carbon performance. Wang et al. [274] modulated the A-site of La 1−x Sr x Fe 0.8 Al 0.2 O 3 oxygen carriers to improve the oxygen content of the oxygen carriers. The experimental results show that after the oxygen carriers were reduced by CH 4 , the modulation of the A-site causes the rapid formation of Fe 0 and RP structure oxide. The RP structure oxide has good oxygen transport properties, so the perovskite and RP structure oxide transferred lattice oxygen rapidly to the Fe 0 , thus suppressing the generation of carbon deposits.
For the suppression of carbon deposition, in addition to modifying the oxygen carrier to accelerate the transmission of lattice oxygen, it can also be achieved by adjusting the reduced properties of the oxygen carrier, such as forming an alloy. It can also avoid the contact of simple metal substances with the reactants through physical isolation, which avoids the formation of carbon deposits in space. The reason for the carbon deposition on the iron-based oxygen carrier is the appearance of Fe 0 . Wang et al. [275] introduced Sn in barium iron perovskite so that the Fe-Sn alloy instead of Fe 0 was in contact with the reducing atmosphere to achieve this purpose. Wang et al. [276] introduced Al into iron-based perovskites so that the oxygen carrier formed a core-shell structure during the reduction process. The formation of core-shell structure after reduction was clearly observed through HRTEM and EDS mapping. The formation of the core-shell structure was attributed to strong metal-support interactions, and the core-shell structure prevented elemental iron from directly contacting CH 4 , thus inhibiting the generation of carbon deposits. The addition of Al achieved the in situ coating of elemental iron, and the resulting double perovskite shell also had good lattice oxygen conductivity. XANES and Mössbauer characterization revealed that Al-doped samples had a higher proportion of Fe 4+ and a lower proportion of oxygen vacancies, indicating that the addition of Al suppressed the generation of oxygen vacancies. DFT calculations showed that Sr and Al co-doped samples could produce two types of oxygen vacancies, namely, Fe-O Vac and Al-O Vac . The E vac of Fe-O Vac was lower than that of Al-O Vac , indicating that the addition of Al inhibited the formation of oxygen vacancies, thus effectively alleviating the production of methane overoxidation.
In addition to La-perovskite, Zhang et al. [277,278] studied the application of SrFe 3−δ perovskite in CLR (Fig. 12). Instead of directly using perovskite as the oxygen carrier, Zhang et al. [277] dispersed SrFe 3−δ perovskite into the CaO dispersing medium to form nanocomposites. By shortening the oxidation time, the average conversion of CH 4 reached 90%, and the conversion of CO 2 in the oxidation stage was maintained at 100%. At the same time, Zhang et al. [278] dispersed perovskite into CaO·MnO, and found that manganese oxide reacted with carbon deposits at high temperatures, which effectively suppressed the carbon deposit selectivity. On this basis, Zhang et al. [279] also used chlorine dopants for SrFeO 3−δ -CaO to improve the performance. The introduction of chlorine promotes the cracking of methane in the reduction process, so that the conversion of CH 4 and CO 2 can reach up to 98% and 100%, respectively, with high carbon efficiency.
In addition to spinel, ilmenite, and perovskite composite oxide oxygen carriers discussed in the previous sections, hexaaluminate structure oxygen carriers have also received close attention due to their structural specificity and high temperature stability [152,280,281]. After the Fe-based oxygen carrier is reduced by CH 4 and reoxidized with air, electrophilic O 2− or O − species are enriched on the surface, thereby reducing the overall CO selectivity. In order to solve this problem, Wang et al. [152] adopted a similar method mentioned in the previous section to control the regeneration extent of oxygen carriers. For the Ba-hexaaluminate oxygen carrier, the oxidation time was shortened, which increased the selectivity of CO by 43% during the methane reduction stage [152]. They further discussed the active sites of methane oxidation and the reason for the increase in selectivity, i.e., Fe 3+ in Al(1), Al(2), and Al(3) sites of BaFe 3 Al 9 O 19 oxygen carrier, which were beneficial to the combustion of methane to generate CO 2 , were reduced, and the amount of Fe 2+ and Fe 0 , which were responsible for CO generation, was increased. Wang et al. [181] further studied the La-hexaaluminate oxygen carrier, and found that O 6 -Fe 3+ (Oh) in the LaFe 3 Al 9 O 19 oxygen carrier had a high activity to completely oxidize methane in the magnetite structure of oxygen carrier activity, while O 5 -Fe 3+ (Tr) and O 4 -Fe 3+ (Th) in the LaFe 3 Al 9 O 19 oxygen carrier selectively oxidized methane to syngas. Interestingly, when CO 2 was used as an oxidant, CO 2 only selectively oxidized O 5 -Fe 3+ (Tr) and O 4 -Fe 3+ (Th), which effectively improved the selectivity of syngas and made effective use of CO 2 . Substituting part of Fe with other metals in BaFe 3 Al 9 O 19 was further studied to optimize the performance of oxygen carriers [282]. Bimetallic BaFe 2 MAl 9 O 19 (M = Mn, Ni, and Co) only crystallized in β-Al 2 O 3 hexaaluminate due to the existence of Mn, Ni, and Co, with + 2 valence state, and the β-Al 2 O 3 structure remained during the CH 4 reduction step. It was found the CO 2 regenerated BaFe 2 CoAl 9 O 19 oxygen

Review
Discover Chemical Engineering (2022) 2:5 | https://doi.org/10.1007/s43938-022-00012-3 1 3 carriers exhibited improved reactivity and cyclic stability for CO 2 utilization and syngas generation with high CH 4 conversion, high syngas yield and desirable H 2 /CO ratio (~ 2). The performance improvement was attributed to the enhanced oxygen-donation ability and the preservation of hexaaluminate phase during successive CH 4 /CO 2 redox cycles. The performance of the oxygen carrier is closely related to the crystal structure of the oxygen carrier, and the necessary calcination temperature guarantees the formation of the target crystal phase, as is the La-Fe-Al hexaaluminate oxygen carrier [281]. When the calcination temperature did not reach the crystal phase formation temperature, the oxygen carriers were mainly iron oxide and perovskite. With increasing calcination temperature to 1100 °C, the crystal structure of the oxygen carrier was hexaaluminate, and there were no impurities. By testing oxygen carriers with different calcination temperatures, it was found that there was a clear difference, which showed that the performance of the hexaaluminate oxygen carrier was related to its crystal structure rather than composition. The hexaaluminate oxygen carrier also has a relatively special property that it can still maintain the original crystal structure after reduction. By comparing the XRD of the fresh oxygen carrier with the reduced oxygen carrier, the XRD peak of the reduced oxygen carrier shifted to a low angle due to the reduction of iron, but it still maintained the MP structure. This property was due to the charge compensation mechanism of hexaaluminate. At the same time, this charge compensation mechanism will also be evident when Al is replaced by different metals [280]. XPS revealed that the doped Mn, Ni and Co metals all existed in the form of divalent ions, so that compared with the undoped oxygen carriers, the XRD results of these doped oxygen carriers were mainly β-Al 2 O 3 because the ideal valence state of large cations in β-Al 2 O 3 was 1.5 and that in MP was 2.4. In most articles, the general focus is on the chemical properties of the oxygen carrier, and the physical properties are only concerned with the specific surface area and the like, but the mechanical properties of the oxygen carrier are also extremely important to it. Good mechanical properties are Fig. 12 a Coproduction of H 2 /CO and CH 3 OH from CH 4 and H 2 O/CO 2 by chemical looping reforming. Reproduced from ref. [278] with permission from the American Chemical Society, copyright 2019. b Redox stability of SrFeO 3−δ -CaO at 980 °C during the chemical looping dry reforming process. Reproduced from ref. [277] with permission from the American Association for the Advancement of Science, copyright 2017. c Redox stability of SrFeO 3−δ /CaO·MnO at 900 °C during the chemical looping steam reforming process. Reproduced from ref. [278] with permission from the American Chemical Society, copyright 2019 1 3 the prerequisite to ensure the normal operation of the oxygen carrier. The mechanical properties of hexaaluminate oxygen carriers doped with different metals were tested, and it was found that the mechanical properties were also related to the doped metals. The advantages of low price and wide sources of iron ores have made the wide applications of Fe-based oxygen carriers more feasible. At present, iron ores have been used in various chemical looping processes, with ilmenite as one successful example for CLC. Lu et al. [283] applied ilmenite and nickel-impregnated ilmenite to the CLR process, and the iron species in ilmenite was also gradually reduced from Fe 3+ to Fe 0 during the reduction process. And when nickel was introduced, the oxygen carrier was reduced to form Ni or Ni-Fe so that syngas was prepared in the presence of CO 2 . Different from the introduction of transition metal oxides, Gu et al. [284] modified natural iron ore with rare earth metals, and found that the introduction of CeO 2 and La 2 O 3 both promoted the reactivity of iron ore, and no carbon deposits were found during the reduction process. The introduction of La 2 O 3 causes the formation of LaFeO 3 after the oxygen carrier is oxidized, which is beneficial to the H 2 production. Lu et al. [285] used magnetite for chemical looping methane reforming and explored the changes of magnetite during the reaction. TGA tests showed that magnetite required a longer induction period to obtain better performance, which was probably related to the dense structure of magnetite. And the presence of only a small amount of CO 2 during the performance test indicated that magnetite oxidized methane to syngas with high selectivity. XRD characterization showed that the crystal phases of magnetite after the reaction were basically the same as those after calcination, which proved the stability of iron ore during the reaction. Further study was conducted and it was found that the temperature of the reduction as well as reoxidation process exerted a great influence on the reactivity and purity of H 2 [286]. Increasing temperature from 800 to 1000 ℃ was beneficial to the reduction of iron oxide which took part in methane activation, and controlling the reoxidation temperature under 650 ℃ would eliminate the effect of carbon impurities (C and Fe 3 C) generated during the reduction process on the purity of H 2 . When the reoxidation was higher than 650 ℃, the steam would react with carbon deposit to form CO and CO 2 , resulting in lower purity of H 2 . Besides, pre-treatment of iron ore was responsible for performance improvement. Iron ore generally needs to be calcined at high temperatures to remove moisture and volatiles before engagement in redox cycles. At the same time, metal hydroxides and carbonates are decomposed, and stable metal oxides are formed after calcination. Therefore, the H 2 yield in the steam oxidation stage of the calcined oxygen carrier was slightly improved compared with that of the original oxygen carrier [285]. Li et al. [287] concluded that ultrasonic treatment also leads to the enhancement of the performance of iron ore, the reason being that ultrasonic action promotes the interaction between the active fractions in iron ore and between the active fractions and the inert material, thus increasing the activity of iron ore. It was also found that during the reduction process of magnetite, the reduction occurs first at the boundary between the active fraction and the inert material, and then gradually spreads to the surrounding area.
Hematite has good activity and stability in the process of methane chemical looping combustion [288], and Gu et al. [289] applied it for CLR and modified it with sunflower straw ash. The results proved that the H 2 yield of the modified iron ore is increased by approximately 1.1 times, and has a better stability. The reason for the good performance was that the sunflower straw ash contained a certain proportion of potassium carbonate, and the addition of potassium carbonate weakened the Fe-O bond. In addition to CH 4 , hematite has also been used in the process of producing H 2 from vegetable oil with desirable performance [290]. Although iron ore has achieved promising results in the application of CLR, problems (low reactivity, sintering, agglomeration and changes in mechanical properties) caused by cycling have also occurred in the process. Huang et al. [291] used hematite for biomass to syngas, and found that the presence of hematite increased the gas yield and carbon conversion by approximately 41%. However, as the number of cycles increased, hematite sintering and abrasion became serious problems. Therefore, the application of iron ore in the chemical looping process needs further research on these aspects.
Although the supported oxygen carrier is more convenient to prepare, it is correspondingly faced with more serious sintering and carbon deposition problems, and the activity of iron oxide needs to be further improved. Although composite oxide oxygen carriers can combine the effects of multiple metals, they also face the disadvantages of poor oxygen storage capacity and structural decomposition. Its application needs further research to obtain oxygen carriers with high activity and selectivity. For naturally occurring iron ore-based oxygen carriers, subsequent research should focus on inhibiting sintering and agglomeration, and improving mechanical properties.

Copper based oxygen carrier
Lewis and Gillil proposed to use the redox cycle between CuO and Cu 2 O for producing food grade CO 2 , which is a typical example of CLOU [48,[292][293][294]. The equilibrium oxygen partial pressure with CuO could be as high as 0.01 bar at 900 °C, which is much higher than that of other types of oxygen carriers and could dramatically promote the carbonaceous fuel gasification and combustion process. Cu-based oxygen carriers have the advantages of high reactivity, high oxygen storage capacity, and low price [133,136]. However, the sintering problem under high-temperature reaction conditions is one of the main reasons limiting its future development in the field of CLR. The literature shows that the reactivity with CH 4 of Cu-based oxygen carriers, although less than that of Ni-based oxygen carriers, was stronger than that of Fe-based and Mn-based oxygen carriers, which proves its potential for development [295]. Therefore, solving the sintering problem of Cu-based oxygen carriers has been the main direction of its further development in chemical looping applications. Both supports and promoters have been tested to alleviate the sintering problem. The addition of inert supports such as Al 2 O 3 [133,[296][297][298], TiO 2 [133,297,299], and MgAl 2 O 4 [300] can slow down the sintering problem of copper oxide, but the addition of Al 2 O 3 , an acidic support, leads to the aggravation of carbon deposition [301]. As a result, Alirezaei et al. [193] incorporated ZrO 2 into Al 2 O 3 , which promoted the dispersion of copper oxide and adjusted the mechanical properties of oxygen carriers. Such modification also effectively suppressed carbon deposits, with the maximum reduction of carbon accumulation by approximately 94%. Instead of alleviating the sintering problem at high reaction temperature, it is an alternative to enhanced oxygen transport capacity of Cu-based oxygen carriers under a lower temperature with alkaline metal oxides, e.g., MgO. Researchers tested the impact of alkaline earth metal oxides, i.e., Mg and Ca, as well as the alkali metal oxides, Na and K oxides, on the enhancement of oxygen uncoupling at lower temperatures. A series of CuO oxygen carriers with 5 wt% of alkali oxides addition were synthesised and studied with thermogravimetric analyzer regarding the oxygen uncoupling behaviour. The results showed that MgO had a positive effect while Na 2 O and K 2 O showed an opposite trend and CaO did not show sensible change on the uncoupling rate at temperature lower than 850 ℃. The clear enhancement of MgO addition was ascribed to its ability to enhance the chemical stability that allows steady oxygen uncoupling [294].
The relatively lower reforming temperature of alcohols can alleviate the sintering problem of copper-based oxygen carriers to some extent. Besides, the excellent performance of Cu-Zn-Al catalysts in traditional alcohol reforming processes for H 2 generation has inspired the exploration of Cu-based oxygen carriers in chemical looping alcohol reforming. For the as-proposed chemical looping oxidative steam reforming of methanol, the Ca 2 Fe 2 O 5 was utilized to support copper oxide to tune the redox activity and achieve a relatively stable catalytic activity. The lattice oxygen concentration is one of the dominant factors determining the methanol conversion pathways and a pathway from formaldehyde intermediate to methyl-formate intermediate was observed with decreasing lattice oxygen concentration by in situ drifts characterization. The introduction of Ca 2 Fe 2 O 5 was aimed at regulating the lattice oxygen's redox activity and mobility, achieving the homogenous release of lattice oxygen. Also, the active copper species were also kept at an appropriate oxidation state to provide compatible active oxygen species for methanol oxidative reforming. The Cu 2 O-Cu looping was accomplished by regulating the reaction temperature and airflow rate, and this proposed lower-valence looping could prevent the excessive oxidation of methanol. During the performance tests, the copper-based catalyst, Cu 2 O-Ca 2 Fe 2 O 5 , showed high catalytic activity with a H 2 production rate of 37.6 µmol H 2 / (g catalyst ·s) under a temperature of 240 °C, as well as an acceptable redox durability within 60 cyclic tests [93]. Wang [113] loaded copper oxide on Al 2 O 3 and used it for ethanol reforming. It was found that the oxygen released by copper oxide promoted the elimination of carbon deposition, and the carbon deposition gradually decreased with the increase of copper oxide when the reaction temperature reached 500 °C. Instead of avoiding carbon deposition, to generate high-purity H 2 with a low concentration of CO, the bi-functional material CuO-MgO was adopted for sorption-enhanced steam methanol reforming. CuO served as an active catalytic site for methanol reforming to H 2 and CO 2 , and CO 2 was removed by MgO sorbent with high-purity H 2 . Also, it was found that the appropriate amount of Cu 2+ entering in MgO lattice could enlarge CO 2 adsorption capacity and enhance CO 2 desorption. Simultaneously, Cu species were significantly dispersed and stabilized due to the existence of MgO [195]. On this basis, sorptionenhanced chemical-looping oxidative steaming reforming of methanol was further proposed and simulated with the Cu-Mg based bifunctional catalyst. In the study, copper species existed in oxidized state and underwent a reduction process in the fuel reactor. Hence, the gradually reduced CuO provided not only catalytic site but lattice oxygen while Mg-based sorbent continued to go through CO 2 adsorption and desorption reactions. The simulation results revealed that CuO and MgO could shift the equilibrium of the WGS reaction and suppress CO generation. And the proposed process achieved auto-thermal operation after operation parameters such as water to methanol ratio and temperature of reactors being analysed and optimized [111,194]. With further addition of Ga 2 O 3 , the catalyst showed strong resistance to particle sintering and agglomeration as the particle size of Cu showed no conspicuous change as evidenced by XRD and TEM characterization after cycles [112]. Without severe sintering problem under a relatively lower alcohol reforming temperature, it could be anticipated that the integration of chemical looping and SER could be a promising strategy to address the carbon deposition issue and achieve high-purity H 2 production from alchols [195]. Fundamental and applied research on copper oxide for low-temperature reforming deserves further effort.

Cerium based oxygen carrier
CeO 2 is a typical representative of the oxygen carrier of fluorite structure. It has been extensively studied in the reactions of CO oxidation, CO 2 hydrogenation, and reforming of methane and alcohols, and has also been successfully applied in three-way catalysts [302,303]. The rapid generation and elimination of oxygen vacancies in CeO 2 makes it a suitable oxygen carrier material [304]. CeO 2 was originally used as an oxygen storage material in automotive three-way catalysts, and the first generation of commercial CeO 2 oxygen storage materials came out in 1989 [305]. The role of CeO 2 is to make the three-way catalyst adapt to different working conditions through the reversible transformation between Ce 4+ and Ce 3+ . At the same time, it can also promote metal dispersion, enhance support stability, and facilitate water gas shift and steam reforming reactions. The role of CeO 2 in this process is similar to that of oxygen carriers in CLR. Then, Otsuka et al. [306] applied CeO 2 catalyst to the field of methane oxidation and successfully obtained a synthesis gas with a H 2 / CO ratio of 2. The successful application of CeO 2 in three-way catalysts and methane oxidation has made it promising for CLR. For CeO 2 , the good oxygen storage capacity and oxygen migration ability render CeO 2 a good choice as dopant or support for oxygen carriers, but when it is used as an oxygen carrier alone, its poor reactivity, low reduction degree, and sintering problems at high temperatures are exposed.
In the three-way catalyst, ZrO 2 was added to CeO 2 to improve the stability and oxygen storage capacity. Although the reactivity of ZrO 2 is not good, temperature programmed reduction and other characterizations show that CeO 2 doped with ZrO 2 improves the oxygen storage capacity, stability, and reducibility of CeO 2 [147]. Therefore, for cerium-based oxygen carriers, ZrO 2 is typically considered to be added to CeO 2 . Otsuka et al. [307] conducted methane reforming test on CeO 2 doped with different proportions of ZrO 2 . The results show that when the doping amount of ZrO 2 was 20%, the yield of H 2 and CO was approximately 1.7 times that of pure CeO 2 , indicating that the addition of ZrO 2 significantly enhanced the reactivity of CeO 2 . On this basis, Zheng et al. [148] prepared CeO 2 -ZrO 2 oxygen carriers with a porous structure at different calcination temperatures. 3DOM structures have been shown to be more likely to form under low-temperature calcination and to enhance the reducibility and activity of CeO 2 -ZrO 2 oxygen carriers. Performance tests showed that the low-temperature calcined oxygen carrier had the highest CH 4 conversion and H 2 yield, and maintained an ordered structure after multiple cycles. Meanwhile, Raman characterization revealed higher I 603 /I 463 ratios of porous CeO 2 -ZrO 2 solid solution compared to nonporous samples, indicating that the porous samples had a higher concentration of oxygen vacancies. Furthermore, the concentration of oxygen vacancies decreased with increasing pore size, proving the effect of pore structure on the oxygen vacancy concentration and reactivity of the CeO 2 -ZrO 2 oxygen carrier [158].
Directly supporting CeO 2 on a support having a 3DOM structure is also an alternative. Macroporous LaFeO 3 loaded with CeO 2 is prepared with the aim of combining the advantages of CeO 2 and LaFeO 3 perovskite to obtain an oxygen carrier with excellent performance, as well as providing a new way to combine Ce-based and Fe-based oxygen carriers [99]. TEM images showed that CeO 2 with particle sizes of 2-3 nm was evenly dispersed on the LaFeO 3 perovskite. Meanwhile, the activity tests showed that the performance of the oxygen carrier remained stable in 30 cycles and that the crystal phase of the oxygen carrier did not change after multiple cycles. Simultaneously, after CeO 2 was supported on the LaFeO 3 perovskite, the reducibility of the oxygen carrier was significantly improved. Fe in the perovskite was inclined to Fe 2+ with the interaction of CeO 2 and the perovskite. Doping with a small amount of Fe causes more oxygen vacancies in CeO 2 while forming a solid solution, which helps improve the activity and stability of CeO 2 . Concerning the development of Ce-Fe oxygen carriers, Li et al. [142] and Zhu et al. [308] have elaborated on it in detail, which is not described here. In addition to doping CeO 2 , analogous to the presence of noble metals in the three-way catalysts, transition metals such as Ni, Fe and Co with suitable catalytic ability can be added to CeO 2 to improve its reactivity [86,114,133,167,174,[309][310][311]. Ni has a high methane activation capacity, and its introduction into CeO 2 greatly increased the reactivity so that the conversion of CH 4 was maintained at 95% with 100% syngas selectivity at 800 °C during the 60 cycles test [165].
Different from doping or loading metals with CeO 2 , Wang et al. [312] introduced tin oxide applied in the oxygen ion conductor to achieve water splitting through the circulation between CeO 2 -SnO 2 and Ce 2 Sn 2 O 7 pyrochlore. Compared with the nonstoichiometric cycle of pure CeO 2 , CeO 2 and SnO 2 were used to generate pyrochlore reversibly, which achieved the goal of Ce 4+ to trivalent cerium, thereby increasing the reduction degree of CeO 2 . On the basis of the Ce 2 Sn 2 O 7 pyrochlore. Wang et al. [166] further explored pyrochlore-type oxides, catalyzed the reaction by using Ni on the surface, and provided lattice oxygen through the reversible cycle of CeO 2 -TiO 2 and Ce 2 Ti 2 O 7 pyrochlore (Fig. 13).

3
The synergistic effect between the surface metal and the oxide support significantly increased the yield of CO and H 2 .
High-resolution transmission electron microscopy (HRTEM) and scanning transmission electron microscopy combined with energy-dispersive X-ray spectroscopy (STEM-EDX) results showed that in the fresh and circulating oxygen carriers, NiO was supported on CeO 2 and TiO 2 , but the CeO 2 and TiO 2 were not uniformly mixed. However, after the oxygen carrier was reduced by methane, the distribution of Ce and Ti was uniform, and the lattice fringes were consistent with pyrochlore, which proved the reversible cycle of CeO 2 -TiO 2 and Ce 2 Ti 2 O 7 pyrochlore. According to DFT calculations, the E vac of Ti-doped CeO 2 was lower than that of pure CeO 2 or TiO 2 . The introduction of TiO 2 weakened the Ce-O bond and promoted the oxygen migration ability of CeO 2 . At the same time, calculations showed that the addition of Ni and the corresponding metal-support interface also promoted methane activation and dissociation of H 2 O or CO 2 . By combining the reversible transformation of CeO 2 -TiO 2 and a specific structural oxide, the catalytic effect of the metal was also fully exerted while Ce 4+ was converted to Ce 3+ , which provided a new design idea for Ce-based oxygen carriers.

Other oxygen carrier
Mn-based oxygen carriers not only have the advantages of low price and environmental friendliness like Fe-based oxygen carriers but also have various valence states (+ 2, + 3, and + 4). Johansson pointed out that the reactivity order of transition metal-based oxygen carriers with CH 4 was Ni > Cu > Mn > Fe, while the crushing strength was opposite, and many studies on Mn-based oxygen carriers have been carried out [295]. Although Mn has many valence states, the available valence states for practical use are very few because MnO 2 and Mn 2 O 3 decompose at 460 and 820 °C, respectively [313]. At the same time, MnO is difficult to be reduced even at elevated temperatures. Therefore, for Mn-based oxygen carriers, the transformation of Mn 3 O 4 to MnO is typically used to achieve the target product. Supported Mn 3 O 4 oxygen carriers are mainly used in the CLC process, and the irreversible salts produced by the reaction between manganese oxide and commonly used supports are the main reason for their limited development. By applying Mn 3 O 4 oxygen carriers with different supports to the CLC process, it is found that although Mn 3 O 4 /ZrO 2 faces structural crack problems due to the phase transition of ZrO 2 , the weak interaction between Mn 3 O 4 and ZrO 2 Fig. 13 a STEM image, b1-b4 the corresponding element-mapping images and c HRTEM images of as-synthesized 5Ni/CeO 2 -TiO 2 . d STEM image, e1-e4 the corresponding element-mapping images and f HRTEM images of 5Ni/CeO 2 -TiO 2 after the CH 4 reduction half cycle. g Schematic of the reaction mechanism for chemical looping steam reforming of methane and chemical looping dry reforming of methane processes over the 5Ni/CeO 2 -TiO 2 oxygen carrier. Reproduced from ref. [166] with permission from the Royal Society of Chemistry, copyright 2019 1 3 makes the oxygen carrier possess high activity and good resistance to carbon deposition [141,[314][315][316]. For CLR, Zrmodified Al 2 O 3 also performed well as a support for Mn-based oxygen carriers [197]. Through XRD characterization, it was found that Zr was possibly inserted into Al 2 O 3 or highly dispersed on Al 2 O 3 and that the formation of MnAl 2 O 4 spinel was restricted. At the same time, by adding CO 2 in the same proportion as CH 4 at the reduction stage, the conversion of CH 4 in the 16 cycles of the optimal oxygen carrier at 650 °C was above 95%, and the carbon deposition was reduced by approximately 50%. In addition to changing the supports, the introduction of promoters could improve the performance of Mn-based oxygen carriers. Bazhenova et al. [317] theoretically explained and analyzed the influence of Fe doping on Mn 2 O 3 at the atomic level by DFT calculations. Since Fe-O bonds were more stable than Mn-O bonds, the addition of Fe made the oxides more stable and changed the electronic structure of the oxides. At the same time, E vac increased with the addition of Fe atoms, and the diffusion barrier changed with the concentration and distribution of Fe atoms. Although a series of explorations have been made on the application of manganese-based oxygen carriers in CLR, it has low selectivity to syngas and needs to increase the reactivity. Shen et al. [318] applied B-substituted LaMn 1−x B x O 3+δ (B = Fe, Co and Ni) perovskites to the chemical looping steam reforming process and investigated the effect of different B-substitutions on the reactivity of oxygen carriers. The experimental results showed that different B-site substitutions promoted the oxygen release rate of LaMnO 3 to a certain extent, with the most obvious effect of nickel. However, nickel-doped oxygen carriers have the problem of carbon accumulation. Meanwhile, Fe and Co substitutions provide more active sites for the reaction, matching the bulk phase lattice oxygen migration rate, so the oxygen carriers show good performance. On this basis, Shen et al. [319] doped the A and B sites of LaMnO 3 perovskite with Sr and Co. The introduction of Sr promoted the migration of lattice oxygen through the generation of oxygen vacancies, while Co in the B-site could provide active sites for the reaction, so that the surface reaction and bulk phase lattice oxygen migration were well matched and the oxygen carrier showed good reaction performance. Research also showed introduction of Cu to B-site was featured with improved performance on carbon formation resistance. Catalysts with various amount of Cu showed different trend for H 2 productivity and resistance for carbon deposition. With increasing Cu content, H 2 productivity saw a rise at first and then dropped, while the amount of carbon deposition displayed a steady upward trend. An appropriate substitution of Cu for La was beneficial for promoting H 2 productivity and reducing carbon deposition and it was attributed to the enhanced reducibility and changes of oxygen species obtained from H 2 -TPR and CH 4 -TPR. [320]. One should also be aware that the amount of doping metal as well as calcination temperature are essential optimization parameters. Yang et al. [321] prepared two series of Fe-doped LaMnO 3 oxygen carriers calcined at temperatures ranging from 700 to 850 ℃. The series of La 0.85 MnFe 0.15 O 3 showed better structural and porous properties, and samples exhibiting higher CH 4 conversion and syngas productivity were with a higher concentration of oxygen vacancies and better oxygen mobility. For both series, La 0.85 MnFe 0.15 O 3 and LaMn 0.9 Fe 0.1 O 3 , different calcined temperature resulted in the shift and intensity of reduction peaks in H 2 -TPR and CH 4 -TPR results, which implied the reducibility degree and oxygen mobility. It was found that two samples, La 0.85 MnFe 0.15 O 3 and LaMn 0.9 Fe 0.1 O 3 , with calcination temperature at 800 ℃, presented ideal ratios of H 2 /CO in the isothermal reaction and larger amount of H 2 during the water splitting step.
The applications of cobalt oxide in chemical looping reported in the literature are mainly as an auxiliary agent to increase the activity and stability of oxygen carriers, including inhibiting the interaction between metal and Al 2 O 3 support, increasing the dispersion of metal to enhance the activity of oxygen carriers, and forming alloys with metal to suppress sintering [126,313]. Although the oxygen carrying capacity of Co 3 O 4 is much higher than that of NiO, Fe 2 O 3 , Mn 2 O 3 and CuO, there are relatively few reports on Co 3 O 4 -based oxygen carriers. Leaving aside its high price, Co 3 O 4 is less active at low temperatures. Its decomposition at 890 °C also limits the increase of reaction temperature because the CoO produced after decomposition has poor reactivity to reactants such as CH 4 , and its reaction with supports (Al 2 O 3 , TiO 2 , and MgO) is also considered to be one of the reasons for the degradation of oxygen carriers' performance [134]. With concerns on the reoxidation of cobalt in the cycling process and the reactivity, the development of cobalt oxide oxygen carriers is limited [322]. A deeper understanding of the phase and surface properties that influence the particle stability and reactivity of Co 3 O 4 during the reaction could help promote its application in chemical looping. On the basis of optimizing the properties of unsupported Co 3 O 4 oxygen carriers, Alalwan et al. [323] carried out a detailed study of the changes in the surface and bulk properties during the reaction process and proposed that the interface between the metal and metal oxide might be helpful to improve Co-based oxygen carriers. The Oxygen carrier was reduced through the path of Co 3 O 4 to CoO and finally to Co, and its performance was enhanced with increasing temperature and decreasing space velocity in the test temperature and gas hourly space velocity range. Importantly, it was found through XRD and XPS characterization showed that the reduction process of CoO to Co followed the nucleation and nuclei growth 1 3 mechanism within the particle bulk. It was mainly because of the lower cohesive energy of oxygen atoms at the interface of these phases that CoO and Co mixtures had better performance. The aluminate or titanate produced through the reaction between cobalt oxide and support during the reduction stage can also be directly used as the oxygen carrier. Wong et al. [200] and Rios et al. [324] took advantage of the stability of aluminates and titanates in Co-based oxygen carriers, and directly applied CoAl 2 O 4 and Co 2 TiO 4 oxygen carriers to chemical looping dry reforming and partial oxidation, respectively. They found through performance tests that although there were some deficiencies in the two oxygen carriers, the results proved the possibility of their applications in CLR. Perovskite structure has also been used in Co-based oxygen carriers due to their excellent high-temperature stability and oxygen migration ability [202,203,325,326]. BaCoO 3-δ /CeO 2 and Ba 1-x Sr x CoO 3-δ /CeO 2 oxygen carriers were used in chemical looping steam methane reforming to investigate the effect of support and A-site doping on the properties of Co-based perovskite oxygen carriers [202,203]. Compared with the BaCoO 3-δ oxygen carrier, the addition of CeO 2 increased the syngas and H 2 yields. During the reduction process, CeO 2 mainly played two roles: one was to form BaCeO 3 with the consumption of BaCoO 3-δ , and the other was to provide oxygen for methane partial oxidation while being reduced to CeO 1.675 . Both of these processes promoted the production of syngas, and the presence of CeO 1.675 also increased the production of H 2 in the steam oxidation stage. After Sr doping, the A-site metal interacted with CeO 2 to reversibly form BaCeO 3 and SrCeO 3 , which was beneficial for the production of syngas and H 2 .
Lee et al. [327] applied B-site substituted LaCo 0.6 B 0.4 O 3 (B = Fe, Mn, Ni) oxygen carriers to the chemical looping steam reforming process and investigated the effects of different B-site substitutions on the performance of oxygen carriers. The experimental results showed that the introduction of iron promoted the oxidation of the oxygen carrier by steam and promoted the migration of lattice oxygen from the bulk phase to the surface oxygen vacancies, so that the LaCo 0.6 Fe 0.4 O 3 oxygen carrier has good reactivity and cyclic stability. Previous studies have shown that Co and Mn-based oxygen carriers are promising candidates, however, their corresponding oxygen partial pressure is more suitable for full oxidation applications, and how to tune their structures and properties for CLR remains challenging.
Tungsten oxides are located in the partial oxidation zone of the Ellingham diagram in Fig. 1, which proves that it is thermodynamically feasible to obtain syngas under a chemical looping fashion. The polyvalent state of WO 3 and its high melting point make it suitable for application in the field of chemical looping. Compared with Fe 2 O 3 , SnO 2 , V 2 O 5 , and MoO 2 oxide, the methane reforming test in a fixed bed at 900 °C found that WO 3 had the highest CO selectivity and the lowest CO 2 selectivity [328]. Both calculations and experiments have proven that W-based oxygen carriers are potential candidates, but the main reasons for the lack of related research are their poor activity and the problem of carbon deposition. To solve these problems, researchers have conducted in-depth studies on the effects of supports and promoters on activity and stability. The activity of WO 3 on supports (Al 2 O 3 , SiO 2 , and ZrO 2 ) was tested, and it was found that the performance of WO 3 /ZrO 2 was significantly improved [204,329]. Further research was carried out on WO 3 /ZrO 2 , and it was found that WO 3 would also be reduced by the syngas produced in the methane reforming stage and that the proportion of H 2 reduction would be greater [330]. Chen et al. [205] introduced NiO to modify WO 3 and improve its reactivity. Bulk doped Ni weakened the strength of the W-O bond to increase the oxygen transfer rate, and surface Ni form reduction was used as the active site for the catalytic methane reaction. The reaction mechanism of WO 3 with CH 4 was obtained through XRD and other characterizations. WO 3 -WO 2.96 and WO 2.96 -WO 2.72 were responsible for full oxidation, and WO 2.72 -WO 2 and WO 2 -W were responsible for partial oxidation. Methane cracking and carbon deposition were caused by metallic Ni and W. The modification of the surface and bulk made its performance much better than that of pure WO 3 . However, its performance and structure gradually changed during ten cycles, which needed further improvement on the stability. In order to improve the activity of the tungsten oxide oxygen carrier and maintain the structural stability of the oxygen carrier during cycling, Liu et al. [206] prepared the Fe y WO x /SiO 2 oxygen carrier and applied it to CLR. The addition of iron greatly improved the performance of the oxygen carrier, and during the reduction process, the strong interaction between iron and tungsten resulted in the formation of the iron-tungsten alloy so that no phase separation occurred, ensuring structural stability. The TPR characterization showed that the reduction temperature of tungsten oxide decreased with the addition of iron, which proved that the addition of iron weakened the W-O bond and made tungsten oxide contribute more oxygen to participate in the reaction. The existence of the form also improves its selectivity. Iron existed in the form of Fe 2+ in the oxygen carrier, which was also beneficial to the improvement of selectivity. The addition of iron to tungsten oxide provided a new strategy for the development of tungsten oxide oxygen carriers.
With the gradual maturity of the chemical looping reforming process, composite metal oxides are currently the mainstream development trend. After extensive literature review and analysis of the XRD data of the oxygen carrier after reduction, it was found that the composite metal oxide can be classified not only according to the active component but also according to its reduced state. The reduced state of the composite metal oxide can be roughly divided into the following six categories. The first type is the solid solution formed after the reduction of oxygen carriers, mainly including Ce-Fe oxygen carriers [191]. The second type is the alloy formed after reduction, including Ni-Fe oxygen carriers [168] and spinel oxygen carriers [266], as well as BaFe 1−x Sn x O 3−δ perovskite [275]. The third type is phase separation after reduction, and the phase separation can be further subdivided into two cases. One case is that the initial state can be recovered after oxidation, which mainly includes perovskite and double perovskite oxygen carriers, and a small part of spinel oxygen carriers [183,184,186,199,268,331]. Another case is that the initial state cannot be recovered after oxidation, mainly including Ni-W and Fe-Ti oxygen carriers [33,143,205]. The fourth type is the composite metal oxide formed after the reduction of oxygen carriers, mainly including CeO 2-x SnO 2 /Ce 2 Sn 2 O 7 , CeO 2 -TiO 2 /Ce 2 Ti 2 O 7 , Ba 1-x Sr x CoO 3−δ /CeO 2 and BaCoO 3−δ /CeO 2 oxygen carriers [166,202,203,312]. The fifth type is the elemental form after reduction, which La 0. 8 [163,332,333]. This type of oxygen carrier will appear simple substances after reduction, but the main frames that are equivalent to the dispersion media remain unchanged. The last type is the oxygen carrier that retains the crystal structure after reduction. This type of oxygen carrier can still maintain the original crystal structure after the loss of oxygen, which is relatively rare, mainly including LaFe 3 Al 9 O 19 hexaaluminate oxygen carriers [152,181,280,281,282]. Although some studies do not show XRD characterization of the oxygen carrier after reduction, which makes some studies cannot be classified better, most of the classifications are currently representative. And for the oxygen carriers that do not show XRD characterization after reduction, it can be judged according to the type of its active material. For example, if the NiO oxygen carrier is doped with iron, an alloy may be formed during the reduction process [168]. The reduction state of the oxygen carrier is classified according to the representative oxygen carrier, but there are exceptions. For example, most of the perovskites undergo phase separation after reduction, but BaFe 1−x Sn x O 3−δ perovskite forms an alloy [275]. Most of the spinel oxygen carriers form alloys after reduction, but Mn 0.5 Fe 0.5 (FeAl)O x undergoes phase separation [334]. The states of the oxygen carriers after reduction are not only to better distinguish the oxygen carrier, but also to predict the performance of the oxygen carriers. This classification can give researchers a general research direction before conducting literature research, for example, the performance advantages of oxygen carriers may be attributed to the formation of forming alloys or solid solutions after reduction. For example, most perovskite oxygen carriers can be restored to the original crystal phase, so the cycle stability is better. Although composite metal oxides can be classified according to the reduced state, at present, there is a lack of research on the mechanism of their different performance after reduction, and further research on the reduced state is needed.

Conclusions and perspectives
Conventional carbonaceous fuel reforming processes are both capital and energy intensive due to the lengthy unit operations. The chemical looping reforming process integrates the reforming reaction and gas-gas separation in one unit operation via the redox cycle of metal oxide-based oxygen carriers, which could potentially evolve as an affordable, clean and efficient alternative for syngas production. The overall reactions of CLR systems are the same as conventional reforming or partial oxidation processes. The rational design of the CLR reactor system could decouple these reactions with the circulation of effective oxygen carriers, and directly produce high-quality syngas (high CO/H 2 concentrations and desirable ratios) without the need for air separation and/or acid gas removal units. The CLR process is also advantageous in terms of exergy efficiency via recuperating the low-grade heat while producing more high-grade heat with the redox operation scheme.
Historical development has shown the evolution of oxygen carriers from naturally occurring ores to synthesized materials, and the development trend of reactor system from fixed bed batch mode operation to continuous circulating fluidized bed reactor design. The high cost in the scaling-up and engineering of high-temperature reactors and the incomprehension in the design and development of oxygen carriers are the main causes for the slow development of these early CLR processes.
The basic schemes of various CLR processes are summarized. The two-reactor autothermal CLR scheme decouples the overall reaction of POX or ATR in two reactors. Endothermic CLR schemes require specific considerations on reactor design with external heating. The super-dry reforming scheme can directly obtain high CO yield from greenhouse gases CH 4 and CO 2 . Three-reactor autothermal CLR schemes have also been developed to directly produce high purity H 2 with in situ CO 2 capture. Such scheme integrates CLC to provide heat for the reforming reaction, thus avoiding external heating. The design and operation of three interconnected reactors requires systematic approach. Issues that need to 1 3 be further addressed include the simultaneous handling of looping particles, oxygen carrier reactivity and recyclability, heat transfer and solid/gas leakage among the reactors.
The syngas selectivity in a CLR process could be affected by many factors, including reaction stoichiometry, thermodynamic equilibrium, surface reaction path and reactor system configuration. The overall reaction stoichiometry determines the syngas selectivity and H 2 :CO ratio as well as the heat balance based on the fuel and oxidant input. The performance of oxygen carriers, typically metal oxides, can be estimated based on their equilibrium oxygen potential at high temperatures. The oxygen potential of various metal oxides could be studied and categorized with ease via the Ellingham diagram or the oxygen partial pressure diagram. Metal oxides in the CLR group can be used for syngas production from various carbonaceous fuels, which can thermodynamically ensure the stable production of high purity syngas while minimizing carbon deposition. Thermodynamic analysis can guide the selection of active components and estimate the syngas selectivity in CLR system.
The reactor system design also plays a critical role in determining the chemical looping process performance. Fixed bed, fluidized bed and moving bed are widely tested operation modes for the reducer. Fixed bed reactors can handle gaseous fuel but require frequent gas switching at high temperatures, which is not suitable for large-scale operation. In addition, the poor heat transfer between gas and solids in the fixed bed reactor could cause hot spots that further lead to sintering and deactivation of oxygen carriers. Therefore, the gas-solid contacting pattern should be carefully considered for the reducer design. The mixed flow pattern mainly occurs in the single-stage fluidized bed reactor, while the countercurrent and cocurrent flow patterns could be achieved in a moving bed or a series of interconnected fluidized bed system. Various fluidized bed configurations, such as bubbling-, turbulent-and spout-fluidized bed operations, have been applied to provide good mixing characteristics and uniform heat transfer in CLC applications. Two CLR processes have been developed using iron-based moving bed reactor system. The cocurrent moving bed reducer design can help achieve high-quality syngas production because the moving bed reducer does not suffer a reduced shale gas conversion and/or undesirable syngas composition due to gas channelling and back mixing of particles with different oxidation states. The countercurrent moving bed design could maximize both fuel gas and iron oxide conversions, which have been proven by various models.
The reaction principle of oxygen carriers generally involves the generation and recombination of oxygen ions and vacancies, their diffusion in the bulk phase, and their reaction with adsorbed species on the surface. Oxygen carriers can be designed to control the rate of lattice oxygen delivery to the surface catalytic site. This facility permits balancing the rate of oxidation and reduction of the catalyst. The properties of the oxygen carrier can be modified to improve its catalytic function as well as to regulate the rate of the diffusion of reactants in the oxygen carriers in order to minimize byproduct generation. The application of catalytically active oxygen carriers has the potential to drastically increase the yield of the reaction products.
The deactivation of oxygen carriers remains the major problem for CLR applications and researchers have made tremendous efforts to solve the problems of sintering, carbon deposition and poor selectivity of oxygen carriers. Supported oxygen carriers and composite oxide oxygen carriers are currently common types of oxygen carriers. Supported oxygen carriers are vastly used in industrial processes, but inevitably, they face severe sintering and other problems. For composite oxide oxygen carriers, perovskite oxygen carriers are the most widely studied type, and their excellent structure leads to high syngas selectivity. Perovskite oxygen carriers, however, have the problem of poor oxygen storage capacity. Various supports, promoters and preparation methods have been adopted to optimize CLR performance of supported and composite oxide oxygen carriers. The development of oxygen carriers will continue toward the understanding and utilization of bimetal-and polymetal-based oxygen carriers. Nevertheless, alleviating the sintering problem and maintaining the stability of oxygen carries by focusing on the modification merely can be challenging at high temperatures. Closer consideration to lowering the reforming temperature with changing feedstocks is an alternative and the development of low-temperature reforming has been encouraged for the CLR process. The development of bio-oil/alcohol reforming is suggested for low-temperature CLR applications, which reduces the difficulties in maintaining the physical and chemical properties of oxygen carriers and engineering the associated reactor system.
At present, research on the reaction mechanism involved in the CLR process is still a challenge. The general explanation of the reaction process is only made by comparing experimental performance or ordinary characterization methods, and there is no detailed exploration of the reaction mechanism in the reaction process. The understanding of the CLR reaction process needs to be further deepened in combination with catalytic science in order to achieve a clear reaction mechanism and develop new processes. The application of thermodynamics and DFT calculations in the screening and theoretical research of oxygen carriers is particularly critical. The combination of characterization techniques on local structure and DFT calculation could provide a deeper understanding of the oxygen carrier while assisting the experimental research. The difference between the performance of the oxygen carriers and the selectivity of the products is explained theoretically by the analysis of the E vac and the energy barrier of the reaction involved in the process. However, the dynamic nature of the oxygen carrier reaction and the large number of atoms involved have also brought challenges to DFT calculations.
With the significant progress made recently in reactor system and oxygen carrier development, CLR technology has great potential to achieve clean, efficient and cost-effective utilization of carbonaceous fuels.